#------------------------------------------------------------------------------
#$Date: 2016-03-25 23:02:06 +0200 (Fri, 25 Mar 2016) $
#$Revision: 180023 $
#$URL: svn://www.crystallography.net/cod/cif/7/03/17/7031780.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7031780
loop_
_publ_author_name
'Liu, Wei'
'Ji, Ying'
'Bao, Xinjian'
'Wang, Ying'
'Li, Benxian'
'Wang, Xiaofeng'
'Zhao, Xudong'
'Liu, Xiaoyang'
'Feng, Shouhua'
_publ_section_title
;
 Novel open-framework europium silicates prepared under high-temperature
 and high-pressure conditions.
;
_journal_issue                   37
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              13892
_journal_page_last               13898
_journal_paper_doi               10.1039/c4dt01707b
_journal_volume                  43
_journal_year                    2014
_chemical_formula_sum            'Eu3 Na15 O36 Si12'
_chemical_formula_weight         1713.81
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           58
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2 2n'
_symmetry_space_group_name_H-M   'P n n m'
_atom_sites_solution_hydrogens   none
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            1
_cell_length_a                   10.7143(9)
_cell_length_b                   7.5271(7)
_cell_length_c                   10.4913(9)
_cell_measurement_reflns_used    4014
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      50.04
_cell_measurement_theta_min      5.48
_cell_volume                     846.10(13)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  CCD
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0192
_diffrn_reflns_av_sigmaI/netI    0.0138
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       12
_diffrn_reflns_limit_l_min       -7
_diffrn_reflns_number            4014
_diffrn_reflns_theta_full        25.02
_diffrn_reflns_theta_max         25.02
_diffrn_reflns_theta_min         2.72
_exptl_absorpt_coefficient_mu    6.244
_exptl_absorpt_correction_T_max  0.732
_exptl_absorpt_correction_T_min  0.515
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            corlourless
_exptl_crystal_density_diffrn    3.363
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       sheet
_exptl_crystal_F_000             810
_exptl_crystal_size_max          0.12
_exptl_crystal_size_mid          0.09
_exptl_crystal_size_min          0.05
_refine_diff_density_max         0.707
_refine_diff_density_min         -0.490
_refine_diff_density_rms         0.161
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.004
_refine_ls_hydrogen_treatment    none
_refine_ls_matrix_type           full
_refine_ls_number_parameters     87
_refine_ls_number_reflns         791
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.004
_refine_ls_R_factor_all          0.0309
_refine_ls_R_factor_gt           0.0288
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0850P)²+3.7000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1068
_refine_ls_wR_factor_ref         0.1094
_reflns_number_gt                736
_reflns_number_total             791
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c4dt01707b2.cif
_cod_data_source_block           x
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from
2011-04-26.

'_exptl_absorpt_correction_type' value 'Multi Scan'
changed to 'multi-scan' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

 Adding full bibliography for 7031780--7031781.cif.
;
_cod_original_sg_symbol_H-M      Pnnm
_cod_database_code               7031780
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'x+1/2, -y+1/2, -z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'-x-1/2, y-1/2, z-1/2'
'x-1/2, -y-1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_group
Eu1 Eu 0.5000 1.0000 0.5000 0.0120(3) Uani 1 4 d S .
Eu2 Eu 0.75180(17) 0.7657(2) 0.0000 0.0180(4) Uani 0.16 2 d SP 1
Eu3 Eu 1.0000 1.0000 0.0000 0.0151(6) Uani 0.18 4 d SP 1
Na2 Na 0.75180(17) 0.7657(2) 0.0000 0.0180(4) Uani 0.84 2 d SP 2
Na3 Na 1.0000 1.0000 0.0000 0.0151(6) Uani 0.82 4 d SP 2
Na1 Na 0.5000 1.0000 0.0000 0.051(2) Uani 1 4 d S .
Na4 Na 0.7605(3) 0.5249(3) 0.2482(3) 0.0287(7) Uani 1 1 d . .
Si1 Si 0.7871(2) 0.7600(2) 0.5000 0.0072(5) Uani 1 2 d S .
Si2 Si 0.99109(12) 0.7870(2) 0.27635(17) 0.0078(4) Uani 1 1 d . .
O1 O 0.7112(5) 0.9408(8) 0.5000 0.0272(14) Uani 1 2 d S .
O2 O 0.7084(5) 0.5816(7) 0.5000 0.0229(13) Uani 1 2 d S .
O3 O 0.8790(5) 0.7503(7) 0.3791(5) 0.0432(15) Uani 1 1 d . .
O4 O 0.9405(4) 0.7150(5) 0.1428(4) 0.0247(10) Uani 1 1 d . .
O5 O 1.0000 1.0000 0.2600(8) 0.057(3) Uani 1 2 d S .
O6 O 1.1172(4) 0.7089(7) 0.3258(4) 0.0354(12) Uani 1 1 d . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Eu Eu -0.1578 3.6682 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O4 Eu1 O4 180.000(1) 3_465 7_766
O4 Eu1 O4 81.5(2) 3_465 8_576
O4 Eu1 O4 98.5(2) 7_766 8_576
O4 Eu1 O4 98.5(2) 3_465 4_655
O4 Eu1 O4 81.5(2) 7_766 4_655
O4 Eu1 O4 180.00(14) 8_576 4_655
O4 Eu1 O1 97.83(15) 3_465 .
O4 Eu1 O1 82.17(16) 7_766 .
O4 Eu1 O1 97.83(15) 8_576 .
O4 Eu1 O1 82.17(16) 4_655 .
O4 Eu1 O1 82.17(16) 3_465 5_676
O4 Eu1 O1 97.83(15) 7_766 5_676
O4 Eu1 O1 82.17(16) 8_576 5_676
O4 Eu1 O1 97.83(15) 4_655 5_676
O1 Eu1 O1 180.000(1) . 5_676
O4 Eu1 Eu2 49.80(10) 3_465 3_465
O4 Eu1 Eu2 130.20(10) 7_766 3_465
O4 Eu1 Eu2 49.80(10) 8_576 3_465
O4 Eu1 Eu2 130.20(10) 4_655 3_465
O1 Eu1 Eu2 131.92(15) . 3_465
O1 Eu1 Eu2 48.08(15) 5_676 3_465
O4 Eu1 Na2 49.80(10) 3_465 3_465
O4 Eu1 Na2 130.20(10) 7_766 3_465
O4 Eu1 Na2 49.80(10) 8_576 3_465
O4 Eu1 Na2 130.20(10) 4_655 3_465
O1 Eu1 Na2 131.92(15) . 3_465
O1 Eu1 Na2 48.08(15) 5_676 3_465
Eu2 Eu1 Na2 0.00(4) 3_465 3_465
O4 Eu1 Na2 130.20(10) 3_465 7_766
O4 Eu1 Na2 49.80(10) 7_766 7_766
O4 Eu1 Na2 130.20(10) 8_576 7_766
O4 Eu1 Na2 49.80(10) 4_655 7_766
O1 Eu1 Na2 48.08(15) . 7_766
O1 Eu1 Na2 131.92(15) 5_676 7_766
Eu2 Eu1 Na2 180.0 3_465 7_766
Na2 Eu1 Na2 180.0 3_465 7_766
O4 Eu1 Eu2 130.20(10) 3_465 7_766
O4 Eu1 Eu2 49.80(10) 7_766 7_766
O4 Eu1 Eu2 130.20(10) 8_576 7_766
O4 Eu1 Eu2 49.80(10) 4_655 7_766
O1 Eu1 Eu2 48.08(15) . 7_766
O1 Eu1 Eu2 131.92(15) 5_676 7_766
Eu2 Eu1 Eu2 180.0 3_465 7_766
Na2 Eu1 Eu2 180.0 3_465 7_766
Na2 Eu1 Eu2 0.00(4) 7_766 7_766
O4 Eu1 Si1 83.24(11) 3_465 .
O4 Eu1 Si1 96.76(11) 7_766 .
O4 Eu1 Si1 83.24(11) 8_576 .
O4 Eu1 Si1 96.76(11) 4_655 .
O1 Eu1 Si1 19.29(15) . .
O1 Eu1 Si1 160.71(15) 5_676 .
Eu2 Eu1 Si1 112.63(4) 3_465 .
Na2 Eu1 Si1 112.63(4) 3_465 .
Na2 Eu1 Si1 67.37(4) 7_766 .
Eu2 Eu1 Si1 67.37(4) 7_766 .
O4 Eu1 Si1 96.76(11) 3_465 5_676
O4 Eu1 Si1 83.24(11) 7_766 5_676
O4 Eu1 Si1 96.76(11) 8_576 5_676
O4 Eu1 Si1 83.24(11) 4_655 5_676
O1 Eu1 Si1 160.71(15) . 5_676
O1 Eu1 Si1 19.29(15) 5_676 5_676
Eu2 Eu1 Si1 67.37(4) 3_465 5_676
Na2 Eu1 Si1 67.37(4) 3_465 5_676
Na2 Eu1 Si1 112.63(4) 7_766 5_676
Eu2 Eu1 Si1 112.63(4) 7_766 5_676
Si1 Eu1 Si1 180.0 . 5_676
O6 Eu2 O6 103.0(3) 8_575 3_465
O6 Eu2 O2 91.63(14) 8_575 7_765
O6 Eu2 O2 91.63(14) 3_465 7_765
O6 Eu2 O1 100.34(16) 8_575 7_755
O6 Eu2 O1 100.34(16) 3_465 7_755
O2 Eu2 O1 160.6(2) 7_765 7_755
O6 Eu2 O4 164.42(17) 8_575 .
O6 Eu2 O4 92.42(16) 3_465 .
O2 Eu2 O4 90.42(15) 7_765 .
O1 Eu2 O4 74.04(14) 7_755 .
O6 Eu2 O4 92.42(16) 8_575 6
O6 Eu2 O4 164.42(17) 3_465 6
O2 Eu2 O4 90.42(15) 7_765 6
O1 Eu2 O4 74.04(14) 7_755 6
O4 Eu2 O4 72.11(19) . 6
O6 Eu2 Na4 54.76(15) 8_575 6
O6 Eu2 Na4 134.98(13) 3_465 6
O2 Eu2 Na4 123.83(5) 7_765 6
O1 Eu2 Na4 55.36(5) 7_755 6
O4 Eu2 Na4 111.95(11) . 6
O4 Eu2 Na4 53.71(11) 6 6
O6 Eu2 Na4 134.98(13) 8_575 .
O6 Eu2 Na4 54.76(15) 3_465 .
O2 Eu2 Na4 123.83(5) 7_765 .
O1 Eu2 Na4 55.36(5) 7_755 .
O4 Eu2 Na4 53.71(11) . .
O4 Eu2 Na4 111.95(11) 6 .
Na4 Eu2 Na4 110.26(9) 6 .
O6 Eu2 Eu3 117.99(11) 8_575 .
O6 Eu2 Eu3 117.99(11) 3_465 .
O2 Eu2 Eu3 46.28(13) 7_765 .
O1 Eu2 Eu3 114.36(14) 7_755 .
O4 Eu2 Eu3 54.61(10) . .
O4 Eu2 Eu3 54.61(10) 6 .
Na4 Eu2 Eu3 106.92(6) 6 .
Na4 Eu2 Eu3 106.92(6) . .
O6 Eu2 Na1 55.84(14) 8_575 .
O6 Eu2 Na1 55.84(14) 3_465 .
O2 Eu2 Na1 66.99(13) 7_765 .
O1 Eu2 Na1 132.37(14) 7_755 .
O4 Eu2 Na1 138.33(9) . .
O4 Eu2 Na1 138.33(9) 6 .
Na4 Eu2 Na1 109.70(6) 6 .
Na4 Eu2 Na1 109.70(6) . .
Eu3 Eu2 Na1 113.27(4) . .
O6 Eu2 Na4 123.74(16) 8_575 4_655
O6 Eu2 Na4 45.40(11) 3_465 4_655
O2 Eu2 Na4 54.74(5) 7_765 4_655
O1 Eu2 Na4 126.33(5) 7_755 4_655
O4 Eu2 Na4 69.39(10) . 4_655
O4 Eu2 Na4 126.44(13) 6 4_655
Na4 Eu2 Na4 178.27(9) 6 4_655
Na4 Eu2 Na4 71.384(8) . 4_655
Eu3 Eu2 Na4 72.87(5) . 4_655
Na1 Eu2 Na4 68.99(5) . 4_655
O6 Eu2 Na4 45.40(11) 8_575 7_765
O6 Eu2 Na4 123.74(16) 3_465 7_765
O2 Eu2 Na4 54.74(5) 7_765 7_765
O1 Eu2 Na4 126.33(5) 7_755 7_765
O4 Eu2 Na4 126.44(13) . 7_765
O4 Eu2 Na4 69.39(10) 6 7_765
Na4 Eu2 Na4 71.384(9) 6 7_765
Na4 Eu2 Na4 178.27(9) . 7_765
Eu3 Eu2 Na4 72.87(5) . 7_765
Na1 Eu2 Na4 68.99(5) . 7_765
Na4 Eu2 Na4 106.97(9) 4_655 7_765
O2 Eu3 O2 180.0 3_565 7_765
O2 Eu3 O4 90.97(15) 3_565 6
O2 Eu3 O4 89.03(15) 7_765 6
O2 Eu3 O4 89.03(15) 3_565 2_775
O2 Eu3 O4 90.97(15) 7_765 2_775
O4 Eu3 O4 180.00(13) 6 2_775
O2 Eu3 O4 90.97(15) 3_565 .
O2 Eu3 O4 89.03(15) 7_765 .
O4 Eu3 O4 67.60(15) 6 .
O4 Eu3 O4 112.40(15) 2_775 .
O2 Eu3 O4 89.03(15) 3_565 5_775
O2 Eu3 O4 90.97(15) 7_765 5_775
O4 Eu3 O4 112.40(15) 6 5_775
O4 Eu3 O4 67.60(15) 2_775 5_775
O4 Eu3 O4 180.00(10) . 5_775
O2 Eu3 O5 90.000(1) 3_565 5_775
O2 Eu3 O5 90.000(1) 7_765 5_775
O4 Eu3 O5 56.20(8) 6 5_775
O4 Eu3 O5 123.80(8) 2_775 5_775
O4 Eu3 O5 123.80(8) . 5_775
O4 Eu3 O5 56.20(8) 5_775 5_775
O2 Eu3 O5 90.0 3_565 .
O2 Eu3 O5 90.0 7_765 .
O4 Eu3 O5 123.80(8) 6 .
O4 Eu3 O5 56.20(8) 2_775 .
O4 Eu3 O5 56.20(8) . .
O4 Eu3 O5 123.80(8) 5_775 .
O5 Eu3 O5 180.000(1) 5_775 .
O2 Eu3 Eu2 131.07(14) 3_565 .
O2 Eu3 Eu2 48.93(14) 7_765 .
O4 Eu3 Eu2 50.40(9) 6 .
O4 Eu3 Eu2 129.60(9) 2_775 .
O4 Eu3 Eu2 50.40(9) . .
O4 Eu3 Eu2 129.60(9) 5_775 .
O5 Eu3 Eu2 90.0 5_775 .
O5 Eu3 Eu2 90.0 . .
O2 Eu3 Eu2 48.93(14) 3_565 5_775
O2 Eu3 Eu2 131.07(14) 7_765 5_775
O4 Eu3 Eu2 129.60(9) 6 5_775
O4 Eu3 Eu2 50.40(9) 2_775 5_775
O4 Eu3 Eu2 129.60(9) . 5_775
O4 Eu3 Eu2 50.40(9) 5_775 5_775
O5 Eu3 Eu2 90.0 5_775 5_775
O5 Eu3 Eu2 90.0 . 5_775
Eu2 Eu3 Eu2 180.0 . 5_775
O2 Eu3 Si2 84.23(7) 3_565 6
O2 Eu3 Si2 95.77(7) 7_765 6
O4 Eu3 Si2 28.51(8) 6 6
O4 Eu3 Si2 151.49(8) 2_775 6
O4 Eu3 Si2 95.42(8) . 6
O4 Eu3 Si2 84.58(8) 5_775 6
O5 Eu3 Si2 28.98(3) 5_775 6
O5 Eu3 Si2 151.02(3) . 6
Eu2 Eu3 Si2 73.06(3) . 6
Eu2 Eu3 Si2 106.94(3) 5_775 6
O2 Eu3 Si2 95.77(7) 3_565 2_775
O2 Eu3 Si2 84.23(7) 7_765 2_775
O4 Eu3 Si2 151.49(8) 6 2_775
O4 Eu3 Si2 28.51(8) 2_775 2_775
O4 Eu3 Si2 84.58(8) . 2_775
O4 Eu3 Si2 95.42(8) 5_775 2_775
O5 Eu3 Si2 151.02(3) 5_775 2_775
O5 Eu3 Si2 28.98(3) . 2_775
Eu2 Eu3 Si2 106.94(3) . 2_775
Eu2 Eu3 Si2 73.06(3) 5_775 2_775
Si2 Eu3 Si2 180.00(6) 6 2_775
O3 Na1 O3 180.00(18) 8_575 4_655
O3 Na1 O3 58.04(19) 8_575 3_465
O3 Na1 O3 121.96(19) 4_655 3_465
O3 Na1 O3 121.96(19) 8_575 7_765
O3 Na1 O3 58.04(19) 4_655 7_765
O3 Na1 O3 180.0 3_465 7_765
O3 Na1 O6 59.07(14) 8_575 8_575
O3 Na1 O6 120.93(14) 4_655 8_575
O3 Na1 O6 97.95(13) 3_465 8_575
O3 Na1 O6 82.05(13) 7_765 8_575
O3 Na1 O6 97.95(13) 8_575 3_465
O3 Na1 O6 82.05(13) 4_655 3_465
O3 Na1 O6 59.07(14) 3_465 3_465
O3 Na1 O6 120.93(14) 7_765 3_465
O6 Na1 O6 84.49(18) 8_575 3_465
O3 Na1 O6 120.93(14) 8_575 4_655
O3 Na1 O6 59.07(14) 4_655 4_655
O3 Na1 O6 82.05(13) 3_465 4_655
O3 Na1 O6 97.95(13) 7_765 4_655
O6 Na1 O6 180.0 8_575 4_655
O6 Na1 O6 95.51(18) 3_465 4_655
O3 Na1 O6 82.05(13) 8_575 7_765
O3 Na1 O6 97.95(13) 4_655 7_765
O3 Na1 O6 120.93(14) 3_465 7_765
O3 Na1 O6 59.07(14) 7_765 7_765
O6 Na1 O6 95.51(18) 8_575 7_765
O6 Na1 O6 180.0 3_465 7_765
O6 Na1 O6 84.49(18) 4_655 7_765
O3 Na1 Si1 32.30(9) 8_575 3_465
O3 Na1 Si1 147.70(9) 4_655 3_465
O3 Na1 Si1 32.30(9) 3_465 3_465
O3 Na1 Si1 147.70(9) 7_765 3_465
O6 Na1 Si1 88.50(9) 8_575 3_465
O6 Na1 Si1 88.50(9) 3_465 3_465
O6 Na1 Si1 91.50(9) 4_655 3_465
O6 Na1 Si1 91.50(9) 7_765 3_465
O3 Na1 Si1 147.70(9) 8_575 7_765
O3 Na1 Si1 32.30(9) 4_655 7_765
O3 Na1 Si1 147.70(9) 3_465 7_765
O3 Na1 Si1 32.30(9) 7_765 7_765
O6 Na1 Si1 91.50(9) 8_575 7_765
O6 Na1 Si1 91.50(9) 3_465 7_765
O6 Na1 Si1 88.50(9) 4_655 7_765
O6 Na1 Si1 88.50(9) 7_765 7_765
Si1 Na1 Si1 180.0 3_465 7_765
O3 Na1 Si2 30.76(10) 8_575 8_575
O3 Na1 Si2 149.24(10) 4_655 8_575
O3 Na1 Si2 81.61(10) 3_465 8_575
O3 Na1 Si2 98.39(10) 7_765 8_575
O6 Na1 Si2 29.28(9) 8_575 8_575
O6 Na1 Si2 96.69(10) 3_465 8_575
O6 Na1 Si2 150.72(9) 4_655 8_575
O6 Na1 Si2 83.31(10) 7_765 8_575
Si1 Na1 Si2 62.38(4) 3_465 8_575
Si1 Na1 Si2 117.62(4) 7_765 8_575
O3 Na1 Si2 149.24(10) 8_575 4_655
O3 Na1 Si2 30.76(10) 4_655 4_655
O3 Na1 Si2 98.39(10) 3_465 4_655
O3 Na1 Si2 81.61(10) 7_765 4_655
O6 Na1 Si2 150.72(9) 8_575 4_655
O6 Na1 Si2 83.31(10) 3_465 4_655
O6 Na1 Si2 29.28(9) 4_655 4_655
O6 Na1 Si2 96.69(10) 7_765 4_655
Si1 Na1 Si2 117.62(4) 3_465 4_655
Si1 Na1 Si2 62.38(4) 7_765 4_655
Si2 Na1 Si2 180.00(4) 8_575 4_655
O6 Na4 O3 92.0(2) 2_765 .
O6 Na4 O6 176.63(13) 2_765 3_465
O3 Na4 O6 86.72(18) . 3_465
O6 Na4 O4 98.29(17) 2_765 .
O3 Na4 O4 59.81(14) . .
O6 Na4 O4 83.74(15) 3_465 .
O6 Na4 O1 95.54(19) 2_765 7_755
O3 Na4 O1 128.80(19) . 7_755
O6 Na4 O1 87.68(18) 3_465 7_755
O4 Na4 O1 69.00(16) . 7_755
O6 Na4 O2 83.99(18) 2_765 .
O3 Na4 O2 58.15(16) . .
O6 Na4 O2 92.69(17) 3_465 .
O4 Na4 O2 117.96(16) . .
O1 Na4 O2 173.04(19) 7_755 .
O6 Na4 O5 121.21(18) 2_765 3_465
O3 Na4 O5 124.27(19) . 3_465
O6 Na4 O5 57.44(12) 3_465 3_465
O4 Na4 O5 138.69(19) . 3_465
O1 Na4 O5 93.8(2) 7_755 3_465
O2 Na4 O5 80.6(2) . 3_465
O6 Na4 O3 84.95(18) 2_765 4_645
O3 Na4 O3 174.60(16) . 4_645
O6 Na4 O3 96.10(16) 3_465 4_645
O4 Na4 O3 125.00(15) . 4_645
O1 Na4 O3 56.08(15) 7_755 4_645
O2 Na4 O3 116.99(17) . 4_645
O5 Na4 O3 54.53(15) 3_465 4_645
O6 Na4 Eu2 137.01(15) 2_765 .
O3 Na4 Eu2 94.45(14) . .
O6 Na4 Eu2 46.26(11) 3_465 .
O4 Na4 Eu2 50.91(10) . .
O1 Na4 Eu2 49.10(13) 7_755 .
O2 Na4 Eu2 134.25(14) . .
O5 Na4 Eu2 89.08(17) 3_465 .
O3 Na4 Eu2 90.82(11) 4_645 .
O6 Na4 Si2 89.97(16) 2_765 .
O3 Na4 Si2 30.77(10) . .
O6 Na4 Si2 90.49(11) 3_465 .
O4 Na4 Si2 30.13(9) . .
O1 Na4 Si2 98.55(15) 7_755 .
O2 Na4 Si2 88.40(13) . .
O5 Na4 Si2 145.13(9) 3_465 .
O3 Na4 Si2 153.29(14) 4_645 .
Eu2 Na4 Si2 75.20(8) . .
O6 Na4 Si1 94.53(16) 2_765 .
O3 Na4 Si1 29.86(11) . .
O6 Na4 Si1 82.80(12) 3_465 .
O4 Na4 Si1 88.92(11) . .
O1 Na4 Si1 156.82(16) 7_755 .
O2 Na4 Si1 29.77(11) . .
O5 Na4 Si1 98.70(18) 3_465 .
O3 Na4 Si1 145.87(13) 4_645 .
Eu2 Na4 Si1 111.42(8) . .
Si2 Na4 Si1 60.61(6) . .
O1 Si1 O2 117.0(3) . .
O1 Si1 O3 110.7(2) . 6_556
O2 Si1 O3 106.7(2) . 6_556
O1 Si1 O3 110.7(2) . .
O2 Si1 O3 106.7(2) . .
O3 Si1 O3 104.2(4) 6_556 .
O1 Si1 Na1 161.5(2) . 3_565
O2 Si1 Na1 81.5(2) . 3_565
O3 Si1 Na1 60.4(2) 6_556 3_565
O3 Si1 Na1 60.4(2) . 3_565
O1 Si1 Na4 115.47(11) . .
O2 Si1 Na4 58.89(8) . .
O3 Si1 Na4 133.0(2) 6_556 .
O3 Si1 Na4 51.42(18) . .
Na1 Si1 Na4 72.95(6) 3_565 .
O1 Si1 Na4 115.47(11) . 6_556
O2 Si1 Na4 58.89(8) . 6_556
O3 Si1 Na4 51.42(18) 6_556 6_556
O3 Si1 Na4 133.0(2) . 6_556
Na1 Si1 Na4 72.95(6) 3_565 6_556
Na4 Si1 Na4 111.71(11) . 6_556
O1 Si1 Na4 53.50(7) . 7_766
O2 Si1 Na4 115.28(12) . 7_766
O3 Si1 Na4 60.2(2) 6_556 7_766
O3 Si1 Na4 137.8(2) . 7_766
Na1 Si1 Na4 120.53(7) 3_565 7_766
Na4 Si1 Na4 165.57(8) . 7_766
Na4 Si1 Na4 70.737(11) 6_556 7_766
O1 Si1 Na4 53.50(7) . 4_655
O2 Si1 Na4 115.28(12) . 4_655
O3 Si1 Na4 137.8(2) 6_556 4_655
O3 Si1 Na4 60.2(2) . 4_655
Na1 Si1 Na4 120.53(7) 3_565 4_655
Na4 Si1 Na4 70.737(11) . 4_655
Na4 Si1 Na4 165.57(8) 6_556 4_655
Na4 Si1 Na4 103.33(11) 7_766 4_655
O1 Si1 Eu1 28.7(2) . .
O2 Si1 Eu1 88.3(2) . .
O3 Si1 Eu1 123.5(2) 6_556 .
O3 Si1 Eu1 123.5(2) . .
Na1 Si1 Eu1 169.80(7) 3_565 .
Na4 Si1 Eu1 101.76(6) . .
Na4 Si1 Eu1 101.76(6) 6_556 .
Na4 Si1 Eu1 64.09(6) 7_766 .
Na4 Si1 Eu1 64.09(6) 4_655 .
O1 Si1 Eu3 91.6(2) . 3_465
O2 Si1 Eu3 25.4(2) . 3_465
O3 Si1 Eu3 119.51(18) 6_556 3_465
O3 Si1 Eu3 119.51(18) . 3_465
Na1 Si1 Eu3 106.91(5) 3_565 3_465
Na4 Si1 Eu3 68.12(6) . 3_465
Na4 Si1 Eu3 68.12(6) 6_556 3_465
Na4 Si1 Eu3 101.11(6) 7_766 3_465
Na4 Si1 Eu3 101.11(6) 4_655 3_465
Eu1 Si1 Eu3 62.89(4) . 3_465
O6 Si2 O4 117.2(2) . .
O6 Si2 O5 111.0(2) . .
O4 Si2 O5 105.3(3) . .
O6 Si2 O3 110.6(3) . .
O4 Si2 O3 105.8(3) . .
O5 Si2 O3 106.3(3) . .
O6 Si2 Na4 118.0(2) . .
O4 Si2 Na4 56.18(17) . .
O5 Si2 Na4 130.75(11) . .
O3 Si2 Na4 52.10(18) . .
O6 Si2 Na1 58.3(2) . 3_565
O4 Si2 Na1 115.18(17) . 3_565
O5 Si2 Na1 138.5(3) . 3_565
O3 Si2 Na1 54.8(2) . 3_565
Na4 Si2 Na1 70.80(6) . 3_565
O6 Si2 Na4 54.4(2) . 3_565
O4 Si2 Na4 112.49(18) . 3_565
O5 Si2 Na4 60.20(7) . 3_565
O3 Si2 Na4 141.5(2) . 3_565
Na4 Si2 Na4 164.06(8) . 3_565
Na1 Si2 Na4 109.20(7) 3_565 3_565
O6 Si2 Na4 162.18(18) . 4_655
O4 Si2 Na4 80.57(17) . 4_655
O5 Si2 Na4 59.55(6) . 4_655
O3 Si2 Na4 62.4(2) . 4_655
Na4 Si2 Na4 71.90(3) . 4_655
Na1 Si2 Na4 117.16(7) 3_565 4_655
Na4 Si2 Na4 119.66(8) 3_565 4_655
O6 Si2 Eu3 116.6(2) . .
O4 Si2 Eu3 53.60(16) . .
O5 Si2 Eu3 54.9(3) . .
O3 Si2 Eu3 132.7(2) . .
Na4 Si2 Eu3 103.97(7) . .
Na1 Si2 Eu3 165.90(6) 3_565 .
Na4 Si2 Eu3 72.08(6) 3_565 .
Na4 Si2 Eu3 71.81(6) 4_655 .
O6 Si2 Eu1 91.07(17) . 3_565
O4 Si2 Eu1 26.22(15) . 3_565
O5 Si2 Eu1 120.4(3) . 3_565
O3 Si2 Eu1 116.50(18) . 3_565
Na4 Si2 Eu1 64.83(6) . 3_565
Na1 Si2 Eu1 100.62(5) 3_565 3_565
Na4 Si2 Eu1 100.05(6) 3_565 3_565
Na4 Si2 Eu1 106.73(6) 4_655 3_565
Eu3 Si2 Eu1 65.60(3) . 3_565
O6 Si2 Eu2 24.29(16) . 3_565
O4 Si2 Eu2 141.49(17) . 3_565
O5 Si2 Eu2 97.5(2) . 3_565
O3 Si2 Eu2 96.8(2) . 3_565
Na4 Si2 Eu2 125.78(7) . 3_565
Na1 Si2 Eu2 55.52(3) 3_565 3_565
Na4 Si2 Eu2 54.34(6) 3_565 3_565
Na4 Si2 Eu2 137.93(7) 4_655 3_565
Eu3 Si2 Eu2 126.13(4) . 3_565
Eu1 Si2 Eu2 115.34(5) 3_565 3_565
Si1 O1 Eu1 132.0(3) . .
Si1 O1 Na2 140.0(3) . 7_766
Eu1 O1 Na2 88.06(19) . 7_766
Si1 O1 Eu2 140.0(3) . 7_766
Eu1 O1 Eu2 88.06(19) . 7_766
Na2 O1 Eu2 0.000(11) 7_766 7_766
Si1 O1 Na4 98.29(14) . 7_766
Eu1 O1 Na4 93.70(14) . 7_766
Na2 O1 Na4 75.54(13) 7_766 7_766
Eu2 O1 Na4 75.54(13) 7_766 7_766
Si1 O1 Na4 98.29(14) . 4_655
Eu1 O1 Na4 93.70(14) . 4_655
Na2 O1 Na4 75.54(13) 7_766 4_655
Eu2 O1 Na4 75.54(13) 7_766 4_655
Na4 O1 Na4 149.8(3) 7_766 4_655
Si1 O2 Na3 137.5(3) . 3_465
Si1 O2 Eu3 137.5(3) . 3_465
Na3 O2 Eu3 0.0 3_465 3_465
Si1 O2 Na2 137.7(3) . 7_756
Na3 O2 Na2 84.79(18) 3_465 7_756
Eu3 O2 Na2 84.79(18) 3_465 7_756
Si1 O2 Eu2 137.7(3) . 7_756
Na3 O2 Eu2 84.79(18) 3_465 7_756
Eu3 O2 Eu2 84.79(18) 3_465 7_756
Na2 O2 Eu2 0.000(12) 7_756 7_756
Si1 O2 Na4 91.34(13) . 6_556
Na3 O2 Na4 98.96(13) 3_465 6_556
Eu3 O2 Na4 98.96(13) 3_465 6_556
Na2 O2 Na4 79.08(13) 7_756 6_556
Eu2 O2 Na4 79.08(13) 7_756 6_556
Si1 O2 Na4 91.34(13) . .
Na3 O2 Na4 98.96(13) 3_465 .
Eu3 O2 Na4 98.96(13) 3_465 .
Na2 O2 Na4 79.08(13) 7_756 .
Eu2 O2 Na4 79.08(13) 7_756 .
Na4 O2 Na4 150.2(3) 6_556 .
Si1 O3 Si2 164.0(3) . .
Si1 O3 Na4 98.7(2) . .
Si2 O3 Na4 97.1(2) . .
Si1 O3 Na1 87.3(2) . 3_565
Si2 O3 Na1 94.5(2) . 3_565
Na4 O3 Na1 91.67(17) . 3_565
Si1 O3 Na4 90.9(2) . 4_655
Si2 O3 Na4 87.4(2) . 4_655
Na4 O3 Na4 88.22(17) . 4_655
Na1 O3 Na4 178.16(19) 3_565 4_655
Si2 O4 Eu1 135.9(2) . 3_565
Si2 O4 Eu2 137.3(2) . .
Eu1 O4 Eu2 86.67(12) 3_565 .
Si2 O4 Na4 93.7(2) . .
Eu1 O4 Na4 95.39(15) 3_565 .
Eu2 O4 Na4 75.38(14) . .
Si2 O4 Eu3 97.90(19) . .
Eu1 O4 Eu3 97.63(14) 3_565 .
Eu2 O4 Eu3 75.00(11) . .
Na4 O4 Eu3 146.75(18) . .
Si2 O5 Si2 167.8(6) . 2_775
Si2 O5 Eu3 96.1(3) . .
Si2 O5 Eu3 96.1(3) 2_775 .
Si2 O5 Na4 90.62(7) . 4_655
Si2 O5 Na4 89.75(7) 2_775 4_655
Eu3 O5 Na4 88.3(2) . 4_655
Si2 O5 Na4 89.75(7) . 3_565
Si2 O5 Na4 90.62(7) 2_775 3_565
Eu3 O5 Na4 88.3(2) . 3_565
Na4 O5 Na4 176.5(4) 4_655 3_565
Si2 O6 Na2 139.7(3) . 3_565
Si2 O6 Eu2 139.7(3) . 3_565
Na2 O6 Eu2 0.0 3_565 3_565
Si2 O6 Na4 130.7(3) . 2_765
Na2 O6 Na4 89.33(16) 3_565 2_765
Eu2 O6 Na4 89.33(16) 3_565 2_765
Si2 O6 Na4 96.9(2) . 3_565
Na2 O6 Na4 78.97(16) 3_565 3_565
Eu2 O6 Na4 78.97(16) 3_565 3_565
Na4 O6 Na4 98.21(17) 2_765 3_565
Si2 O6 Na1 92.4(2) . 3_565
Na2 O6 Na1 78.84(15) 3_565 3_565
Eu2 O6 Na1 78.84(15) 3_565 3_565
Na4 O6 Na1 93.28(18) 2_765 3_565
Na4 O6 Na1 154.83(19) 3_565 3_565
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Eu1 O4 2.295(4) 3_465
Eu1 O4 2.295(4) 7_766
Eu1 O4 2.295(4) 8_576
Eu1 O4 2.295(4) 4_655
Eu1 O1 2.307(5) .
Eu1 O1 2.307(5) 5_676
Eu1 Eu2 3.3272(16) 3_465
Eu1 Na2 3.3272(16) 3_465
Eu1 Na2 3.3272(16) 7_766
Eu1 Eu2 3.3272(16) 7_766
Eu1 Si1 3.567(2) .
Eu1 Si1 3.567(2) 5_676
Eu2 O6 2.336(4) 8_575
Eu2 O6 2.336(4) 3_465
Eu2 O2 2.416(6) 7_765
Eu2 O1 2.477(6) 7_755
Eu2 O4 2.545(4) .
Eu2 O4 2.545(4) 6
Eu2 Na4 3.173(3) 6
Eu2 Na4 3.173(3) .
Eu2 Eu3 3.1910(18) .
Eu2 Na1 3.2233(17) .
Eu2 Na4 3.287(3) 4_655
Eu2 Na4 3.287(3) 7_765
Eu3 O2 2.316(5) 3_565
Eu3 O2 2.316(5) 7_765
Eu3 O4 2.693(4) 6
Eu3 O4 2.693(4) 2_775
Eu3 O4 2.693(4) .
Eu3 O4 2.693(4) 5_775
Eu3 O5 2.727(9) 5_775
Eu3 O5 2.727(9) .
Eu3 Eu2 3.1910(18) 5_775
Eu3 Si2 3.3144(18) 6
Eu3 Si2 3.3144(18) 2_775
Na1 O3 2.615(6) 8_575
Na1 O3 2.615(6) 4_655
Na1 O3 2.615(6) 3_465
Na1 O3 2.615(6) 7_765
Na1 O6 2.719(6) 8_575
Na1 O6 2.719(6) 3_465
Na1 O6 2.719(6) 4_655
Na1 O6 2.719(6) 7_765
Na1 Si1 3.005(2) 3_465
Na1 Si1 3.005(2) 7_765
Na1 Si2 3.1909(18) 8_575
Na1 Si2 3.1909(18) 4_655
Na4 O6 2.341(5) 2_765
Na4 O3 2.525(5) .
Na4 O6 2.641(6) 3_465
Na4 O4 2.643(5) .
Na4 O1 2.696(3) 7_755
Na4 O2 2.734(3) .
Na4 O5 2.799(3) 3_465
Na4 O3 2.880(6) 4_645
Na4 Si2 3.175(3) .
Na4 Si1 3.192(3) .
Si1 O1 1.585(6) .
Si1 O2 1.586(5) .
Si1 O3 1.608(4) 6_556
Si1 O3 1.608(4) .
Si1 Na1 3.005(2) 3_565
Si1 Na4 3.192(3) 6_556
Si1 Na4 3.319(3) 7_766
Si1 Na4 3.319(3) 4_655
Si1 Eu3 3.646(2) 3_465
Si2 O6 1.562(4) .
Si2 O4 1.597(4) .
Si2 O5 1.615(2) .
Si2 O3 1.637(4) .
Si2 Na1 3.1909(18) 3_565
Si2 Na4 3.226(3) 3_565
Si2 Na4 3.247(3) 4_655
Si2 Eu1 3.6169(18) 3_565
Si2 Eu2 3.670(2) 3_565
O1 Na2 2.477(6) 7_766
O1 Eu2 2.477(6) 7_766
O1 Na4 2.696(3) 7_766
O1 Na4 2.696(3) 4_655
O2 Na3 2.316(5) 3_465
O2 Eu3 2.316(5) 3_465
O2 Na2 2.416(6) 7_756
O2 Eu2 2.416(6) 7_756
O2 Na4 2.734(3) 6_556
O3 Na1 2.615(6) 3_565
O3 Na4 2.880(6) 4_655
O4 Eu1 2.295(4) 3_565
O5 Si2 1.615(2) 2_775
O5 Na4 2.799(3) 4_655
O5 Na4 2.799(3) 3_565
O6 Na2 2.336(4) 3_565
O6 Eu2 2.336(4) 3_565
O6 Na4 2.341(5) 2_765
O6 Na4 2.641(6) 3_565
O6 Na1 2.719(6) 3_565
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
O6 Eu2 Eu3 O2 -117.62(16) 8_575 3_565
O6 Eu2 Eu3 O2 117.62(16) 3_465 3_565
O2 Eu2 Eu3 O2 180.0 7_765 3_565
O1 Eu2 Eu3 O2 0.0 7_755 3_565
O4 Eu2 Eu3 O2 46.22(11) . 3_565
O4 Eu2 Eu3 O2 -46.22(11) 6 3_565
Na4 Eu2 Eu3 O2 -59.04(5) 6 3_565
Na4 Eu2 Eu3 O2 59.04(5) . 3_565
Na1 Eu2 Eu3 O2 180.0 . 3_565
Na4 Eu2 Eu3 O2 122.75(5) 4_655 3_565
Na4 Eu2 Eu3 O2 -122.75(5) 7_765 3_565
O6 Eu2 Eu3 O2 62.38(16) 8_575 7_765
O6 Eu2 Eu3 O2 -62.38(16) 3_465 7_765
O1 Eu2 Eu3 O2 180.0 7_755 7_765
O4 Eu2 Eu3 O2 -133.78(11) . 7_765
O4 Eu2 Eu3 O2 133.78(11) 6 7_765
Na4 Eu2 Eu3 O2 120.96(5) 6 7_765
Na4 Eu2 Eu3 O2 -120.96(5) . 7_765
Na1 Eu2 Eu3 O2 0.0 . 7_765
Na4 Eu2 Eu3 O2 -57.25(5) 4_655 7_765
Na4 Eu2 Eu3 O2 57.25(5) 7_765 7_765
O6 Eu2 Eu3 O4 -71.40(19) 8_575 6
O6 Eu2 Eu3 O4 163.8(2) 3_465 6
O2 Eu2 Eu3 O4 -133.78(11) 7_765 6
O1 Eu2 Eu3 O4 46.22(11) 7_755 6
O4 Eu2 Eu3 O4 92.4(2) . 6
Na4 Eu2 Eu3 O4 -12.82(11) 6 6
Na4 Eu2 Eu3 O4 105.26(12) . 6
Na1 Eu2 Eu3 O4 -133.78(11) . 6
Na4 Eu2 Eu3 O4 168.97(12) 4_655 6
Na4 Eu2 Eu3 O4 -76.53(11) 7_765 6
O6 Eu2 Eu3 O4 108.60(19) 8_575 2_775
O6 Eu2 Eu3 O4 -16.2(2) 3_465 2_775
O2 Eu2 Eu3 O4 46.22(11) 7_765 2_775
O1 Eu2 Eu3 O4 -133.78(11) 7_755 2_775
O4 Eu2 Eu3 O4 -87.6(2) . 2_775
O4 Eu2 Eu3 O4 180.0 6 2_775
Na4 Eu2 Eu3 O4 167.18(11) 6 2_775
Na4 Eu2 Eu3 O4 -74.74(12) . 2_775
Na1 Eu2 Eu3 O4 46.22(11) . 2_775
Na4 Eu2 Eu3 O4 -11.03(12) 4_655 2_775
Na4 Eu2 Eu3 O4 103.47(11) 7_765 2_775
O6 Eu2 Eu3 O4 -163.8(2) 8_575 .
O6 Eu2 Eu3 O4 71.40(19) 3_465 .
O2 Eu2 Eu3 O4 133.78(11) 7_765 .
O1 Eu2 Eu3 O4 -46.22(11) 7_755 .
O4 Eu2 Eu3 O4 -92.4(2) 6 .
Na4 Eu2 Eu3 O4 -105.26(12) 6 .
Na4 Eu2 Eu3 O4 12.82(11) . .
Na1 Eu2 Eu3 O4 133.78(11) . .
Na4 Eu2 Eu3 O4 76.53(11) 4_655 .
Na4 Eu2 Eu3 O4 -168.97(12) 7_765 .
O6 Eu2 Eu3 O4 16.2(2) 8_575 5_775
O6 Eu2 Eu3 O4 -108.60(19) 3_465 5_775
O2 Eu2 Eu3 O4 -46.22(11) 7_765 5_775
O1 Eu2 Eu3 O4 133.78(11) 7_755 5_775
O4 Eu2 Eu3 O4 180.0 . 5_775
O4 Eu2 Eu3 O4 87.6(2) 6 5_775
Na4 Eu2 Eu3 O4 74.74(12) 6 5_775
Na4 Eu2 Eu3 O4 -167.18(11) . 5_775
Na1 Eu2 Eu3 O4 -46.22(11) . 5_775
Na4 Eu2 Eu3 O4 -103.47(11) 4_655 5_775
Na4 Eu2 Eu3 O4 11.03(12) 7_765 5_775
O6 Eu2 Eu3 O5 -27.62(16) 8_575 5_775
O6 Eu2 Eu3 O5 -152.38(16) 3_465 5_775
O2 Eu2 Eu3 O5 -90.0 7_765 5_775
O1 Eu2 Eu3 O5 90.0 7_755 5_775
O4 Eu2 Eu3 O5 136.22(11) . 5_775
O4 Eu2 Eu3 O5 43.78(11) 6 5_775
Na4 Eu2 Eu3 O5 30.96(5) 6 5_775
Na4 Eu2 Eu3 O5 149.04(5) . 5_775
Na1 Eu2 Eu3 O5 -90.0 . 5_775
Na4 Eu2 Eu3 O5 -147.25(5) 4_655 5_775
Na4 Eu2 Eu3 O5 -32.75(5) 7_765 5_775
O6 Eu2 Eu3 O5 152.38(16) 8_575 .
O6 Eu2 Eu3 O5 27.62(16) 3_465 .
O2 Eu2 Eu3 O5 90.0 7_765 .
O1 Eu2 Eu3 O5 -90.0 7_755 .
O4 Eu2 Eu3 O5 -43.78(11) . .
O4 Eu2 Eu3 O5 -136.22(11) 6 .
Na4 Eu2 Eu3 O5 -149.04(5) 6 .
Na4 Eu2 Eu3 O5 -30.96(5) . .
Na1 Eu2 Eu3 O5 90.0 . .
Na4 Eu2 Eu3 O5 32.75(5) 4_655 .
Na4 Eu2 Eu3 O5 147.25(5) 7_765 .
O6 Eu2 Eu3 Eu2 62.38(16) 8_575 5_775
O6 Eu2 Eu3 Eu2 -62.38(16) 3_465 5_775
O2 Eu2 Eu3 Eu2 0.0 7_765 5_775
O1 Eu2 Eu3 Eu2 180.0 7_755 5_775
O4 Eu2 Eu3 Eu2 -133.78(11) . 5_775
O4 Eu2 Eu3 Eu2 133.78(11) 6 5_775
Na4 Eu2 Eu3 Eu2 120.96(5) 6 5_775
Na4 Eu2 Eu3 Eu2 -120.96(5) . 5_775
Na1 Eu2 Eu3 Eu2 0.0 . 5_775
Na4 Eu2 Eu3 Eu2 -57.25(5) 4_655 5_775
Na4 Eu2 Eu3 Eu2 57.25(5) 7_765 5_775
O6 Eu2 Eu3 Si2 -51.50(17) 8_575 6
O6 Eu2 Eu3 Si2 -176.25(17) 3_465 6
O2 Eu2 Eu3 Si2 -113.87(3) 7_765 6
O1 Eu2 Eu3 Si2 66.13(3) 7_755 6
O4 Eu2 Eu3 Si2 112.35(11) . 6
O4 Eu2 Eu3 Si2 19.90(11) 6 6
Na4 Eu2 Eu3 Si2 7.08(5) 6 6
Na4 Eu2 Eu3 Si2 125.17(7) . 6
Na1 Eu2 Eu3 Si2 -113.87(3) . 6
Na4 Eu2 Eu3 Si2 -171.12(7) 4_655 6
Na4 Eu2 Eu3 Si2 -56.63(5) 7_765 6
O6 Eu2 Eu3 Si2 128.50(17) 8_575 2_775
O6 Eu2 Eu3 Si2 3.75(17) 3_465 2_775
O2 Eu2 Eu3 Si2 66.13(3) 7_765 2_775
O1 Eu2 Eu3 Si2 -113.87(3) 7_755 2_775
O4 Eu2 Eu3 Si2 -67.65(11) . 2_775
O4 Eu2 Eu3 Si2 -160.10(11) 6 2_775
Na4 Eu2 Eu3 Si2 -172.92(5) 6 2_775
Na4 Eu2 Eu3 Si2 -54.83(7) . 2_775
Na1 Eu2 Eu3 Si2 66.13(3) . 2_775
Na4 Eu2 Eu3 Si2 8.88(7) 4_655 2_775
Na4 Eu2 Eu3 Si2 123.37(5) 7_765 2_775
O6 Eu2 Na4 O6 109.7(4) 8_575 2_765
O6 Eu2 Na4 O6 -178.9(3) 3_465 2_765
O2 Eu2 Na4 O6 -114.4(3) 7_765 2_765
O1 Eu2 Na4 O6 42.1(3) 7_755 2_765
O4 Eu2 Na4 O6 -53.2(3) . 2_765
O4 Eu2 Na4 O6 -8.2(3) 6 2_765
Na4 Eu2 Na4 O6 49.7(3) 6 2_765
Eu3 Eu2 Na4 O6 -66.2(3) . 2_765
Na1 Eu2 Na4 O6 170.6(2) . 2_765
Na4 Eu2 Na4 O6 -130.9(3) 4_655 2_765
Na4 Eu2 Na4 O6 -149(2) 7_765 2_765
O6 Eu2 Na4 O3 -152.6(2) 8_575 .
O6 Eu2 Na4 O3 -81.15(19) 3_465 .
O2 Eu2 Na4 O3 -16.7(2) 7_765 .
O1 Eu2 Na4 O3 139.8(2) 7_755 .
O4 Eu2 Na4 O3 44.51(16) . .
O4 Eu2 Na4 O3 89.53(17) 6 .
Na4 Eu2 Na4 O3 147.42(13) 6 .
Eu3 Eu2 Na4 O3 31.54(14) . .
Na1 Eu2 Na4 O3 -91.65(14) . .
Na4 Eu2 Na4 O3 -33.16(12) 4_655 .
Na4 Eu2 Na4 O3 -51(2) 7_765 .
O6 Eu2 Na4 O6 -71.5(3) 8_575 3_465
O2 Eu2 Na4 O6 64.4(2) 7_765 3_465
O1 Eu2 Na4 O6 -139.0(2) 7_755 3_465
O4 Eu2 Na4 O6 125.66(18) . 3_465
O4 Eu2 Na4 O6 170.68(18) 6 3_465
Na4 Eu2 Na4 O6 -131.43(15) 6 3_465
Eu3 Eu2 Na4 O6 112.69(13) . 3_465
Na1 Eu2 Na4 O6 -10.51(13) . 3_465
Na4 Eu2 Na4 O6 47.99(13) 4_655 3_465
Na4 Eu2 Na4 O6 30(2) 7_765 3_465
O6 Eu2 Na4 O4 162.9(2) 8_575 .
O6 Eu2 Na4 O4 -125.66(18) 3_465 .
O2 Eu2 Na4 O4 -61.2(2) 7_765 .
O1 Eu2 Na4 O4 95.32(19) 7_755 .
O4 Eu2 Na4 O4 45.02(15) 6 .
Na4 Eu2 Na4 O4 102.91(14) 6 .
Eu3 Eu2 Na4 O4 -12.97(11) . .
Na1 Eu2 Na4 O4 -136.17(12) . .
Na4 Eu2 Na4 O4 -77.67(13) 4_655 .
Na4 Eu2 Na4 O4 -96(2) 7_765 .
O6 Eu2 Na4 O1 67.5(3) 8_575 7_755
O6 Eu2 Na4 O1 139.0(2) 3_465 7_755
O2 Eu2 Na4 O1 -156.5(2) 7_765 7_755
O4 Eu2 Na4 O1 -95.32(19) . 7_755
O4 Eu2 Na4 O1 -50.3(2) 6 7_755
Na4 Eu2 Na4 O1 7.59(19) 6 7_755
Eu3 Eu2 Na4 O1 -108.29(16) . 7_755
Na1 Eu2 Na4 O1 128.51(17) . 7_755
Na4 Eu2 Na4 O1 -172.99(19) 4_655 7_755
Na4 Eu2 Na4 O1 169(2) 7_765 7_755
O6 Eu2 Na4 O2 -104.2(3) 8_575 .
O6 Eu2 Na4 O2 -32.7(2) 3_465 .
O2 Eu2 Na4 O2 31.7(4) 7_765 .
O1 Eu2 Na4 O2 -171.7(3) 7_755 .
O4 Eu2 Na4 O2 93.0(2) . .
O4 Eu2 Na4 O2 138.0(2) 6 .
Na4 Eu2 Na4 O2 -164.12(17) 6 .
Eu3 Eu2 Na4 O2 80.0(2) . .
Na1 Eu2 Na4 O2 -43.2(2) . .
Na4 Eu2 Na4 O2 15.31(17) 4_655 .
Na4 Eu2 Na4 O2 -3(2) 7_765 .
O6 Eu2 Na4 O5 -28.3(2) 8_575 3_465
O6 Eu2 Na4 O5 43.16(17) 3_465 3_465
O2 Eu2 Na4 O5 107.6(2) 7_765 3_465
O1 Eu2 Na4 O5 -95.9(2) 7_755 3_465
O4 Eu2 Na4 O5 168.82(17) . 3_465
O4 Eu2 Na4 O5 -146.17(16) 6 3_465
Na4 Eu2 Na4 O5 -88.27(15) 6 3_465
Eu3 Eu2 Na4 O5 155.85(12) . 3_465
Na1 Eu2 Na4 O5 32.65(13) . 3_465
Na4 Eu2 Na4 O5 91.15(14) 4_655 3_465
Na4 Eu2 Na4 O5 73(2) 7_765 3_465
O6 Eu2 Na4 O3 26.2(2) 8_575 4_645
O6 Eu2 Na4 O3 97.67(18) 3_465 4_645
O2 Eu2 Na4 O3 162.10(19) 7_765 4_645
O1 Eu2 Na4 O3 -41.35(18) 7_755 4_645
O4 Eu2 Na4 O3 -136.67(16) . 4_645
O4 Eu2 Na4 O3 -91.66(16) 6 4_645
Na4 Eu2 Na4 O3 -33.77(15) 6 4_645
Eu3 Eu2 Na4 O3 -149.64(11) . 4_645
Na1 Eu2 Na4 O3 87.16(11) . 4_645
Na4 Eu2 Na4 O3 145.66(15) 4_655 4_645
Na4 Eu2 Na4 O3 128(2) 7_765 4_645
O6 Eu2 Na4 Si2 -176.8(2) 8_575 .
O6 Eu2 Na4 Si2 -105.37(14) 3_465 .
O2 Eu2 Na4 Si2 -40.94(18) 7_765 .
O1 Eu2 Na4 Si2 115.61(17) 7_755 .
O4 Eu2 Na4 Si2 20.29(11) . .
O4 Eu2 Na4 Si2 65.30(12) 6 .
Na4 Eu2 Na4 Si2 123.20(8) 6 .
Eu3 Eu2 Na4 Si2 7.32(6) . .
Na1 Eu2 Na4 Si2 -115.88(6) . .
Na4 Eu2 Na4 Si2 -57.38(6) 4_655 .
Na4 Eu2 Na4 Si2 -75(2) 7_765 .
O6 Eu2 Na4 Si1 -127.3(2) 8_575 .
O6 Eu2 Na4 Si1 -55.83(15) 3_465 .
O2 Eu2 Na4 Si1 8.6(2) 7_765 .
O1 Eu2 Na4 Si1 165.15(19) 7_755 .
O4 Eu2 Na4 Si1 69.83(13) . .
O4 Eu2 Na4 Si1 114.85(13) 6 .
Na4 Eu2 Na4 Si1 172.74(5) 6 .
Eu3 Eu2 Na4 Si1 56.86(9) . .
Na1 Eu2 Na4 Si1 -66.33(10) . .
Na4 Eu2 Na4 Si1 -7.84(6) 4_655 .
Na4 Eu2 Na4 Si1 -26(2) 7_765 .
O6 Na4 Si1 O1 -177.0(3) 2_765 .
O3 Na4 Si1 O1 96.9(4) . .
O6 Na4 Si1 O1 0.9(2) 3_465 .
O4 Na4 Si1 O1 84.8(2) . .
O1 Na4 Si1 O1 67.4(6) 7_755 .
O2 Na4 Si1 O1 -107.5(4) . .
O5 Na4 Si1 O1 -54.5(3) 3_465 .
O3 Na4 Si1 O1 -89.3(3) 4_645 .
Eu2 Na4 Si1 O1 38.0(2) . .
Si2 Na4 Si1 O1 95.6(2) . .
O6 Na4 Si1 O2 -69.5(3) 2_765 .
O3 Na4 Si1 O2 -155.6(4) . .
O6 Na4 Si1 O2 108.4(3) 3_465 .
O4 Na4 Si1 O2 -167.8(3) . .
O1 Na4 Si1 O2 174.9(4) 7_755 .
O5 Na4 Si1 O2 53.0(3) 3_465 .
O3 Na4 Si1 O2 18.2(3) 4_645 .
Eu2 Na4 Si1 O2 145.5(3) . .
Si2 Na4 Si1 O2 -156.9(3) . .
O6 Na4 Si1 O3 14.5(3) 2_765 6_556
O3 Na4 Si1 O3 -71.6(4) . 6_556
O6 Na4 Si1 O3 -167.6(3) 3_465 6_556
O4 Na4 Si1 O3 -83.7(3) . 6_556
O1 Na4 Si1 O3 -101.1(5) 7_755 6_556
O2 Na4 Si1 O3 84.0(4) . 6_556
O5 Na4 Si1 O3 137.0(3) 3_465 6_556
O3 Na4 Si1 O3 102.2(4) 4_645 6_556
Eu2 Na4 Si1 O3 -130.5(3) . 6_556
Si2 Na4 Si1 O3 -72.9(3) . 6_556
O6 Na4 Si1 O3 86.1(3) 2_765 .
O6 Na4 Si1 O3 -96.0(3) 3_465 .
O4 Na4 Si1 O3 -12.1(3) . .
O1 Na4 Si1 O3 -29.5(5) 7_755 .
O2 Na4 Si1 O3 155.6(4) . .
O5 Na4 Si1 O3 -151.4(3) 3_465 .
O3 Na4 Si1 O3 173.8(3) 4_645 .
Eu2 Na4 Si1 O3 -58.9(3) . .
Si2 Na4 Si1 O3 -1.3(3) . .
O6 Na4 Si1 Na1 20.74(13) 2_765 3_565
O3 Na4 Si1 Na1 -65.4(3) . 3_565
O6 Na4 Si1 Na1 -161.33(12) 3_465 3_565
O4 Na4 Si1 Na1 -77.50(11) . 3_565
O1 Na4 Si1 Na1 -94.8(4) 7_755 3_565
O2 Na4 Si1 Na1 90.3(2) . 3_565
O5 Na4 Si1 Na1 143.28(14) 3_465 3_565
O3 Na4 Si1 Na1 108.4(2) 4_645 3_565
Eu2 Na4 Si1 Na1 -124.28(9) . 3_565
Si2 Na4 Si1 Na1 -66.68(6) . 3_565
O6 Na4 Si1 Na4 -42.38(19) 2_765 6_556
O3 Na4 Si1 Na4 -128.5(3) . 6_556
O6 Na4 Si1 Na4 135.55(12) 3_465 6_556
O4 Na4 Si1 Na4 -140.62(11) . 6_556
O1 Na4 Si1 Na4 -157.9(4) 7_755 6_556
O2 Na4 Si1 Na4 27.1(3) . 6_556
O5 Na4 Si1 Na4 80.17(15) 3_465 6_556
O3 Na4 Si1 Na4 45.3(3) 4_645 6_556
Eu2 Na4 Si1 Na4 172.60(5) . 6_556
Si2 Na4 Si1 Na4 -129.79(10) . 6_556
O6 Na4 Si1 Na4 -139.4(4) 2_765 7_766
O3 Na4 Si1 Na4 134.5(5) . 7_766
O6 Na4 Si1 Na4 38.5(4) 3_465 7_766
O4 Na4 Si1 Na4 122.3(4) . 7_766
O1 Na4 Si1 Na4 105.0(5) 7_755 7_766
O2 Na4 Si1 Na4 -69.9(5) . 7_766
O5 Na4 Si1 Na4 -16.9(5) 3_465 7_766
O3 Na4 Si1 Na4 -51.7(6) 4_645 7_766
Eu2 Na4 Si1 Na4 75.6(4) . 7_766
Si2 Na4 Si1 Na4 133.2(4) . 7_766
O6 Na4 Si1 Na4 152.80(18) 2_765 4_655
O3 Na4 Si1 Na4 66.7(3) . 4_655
O6 Na4 Si1 Na4 -29.26(10) 3_465 4_655
O4 Na4 Si1 Na4 54.57(11) . 4_655
O1 Na4 Si1 Na4 37.3(4) 7_755 4_655
O2 Na4 Si1 Na4 -137.7(3) . 4_655
O5 Na4 Si1 Na4 -84.65(14) 3_465 4_655
O3 Na4 Si1 Na4 -119.5(3) 4_645 4_655
Eu2 Na4 Si1 Na4 7.79(5) . 4_655
Si2 Na4 Si1 Na4 65.39(8) . 4_655
O6 Na4 Si1 Eu1 -150.26(14) 2_765 .
O3 Na4 Si1 Eu1 123.7(3) . .
O6 Na4 Si1 Eu1 27.68(11) 3_465 .
O4 Na4 Si1 Eu1 111.51(11) . .
O1 Na4 Si1 Eu1 94.2(4) 7_755 .
O2 Na4 Si1 Eu1 -80.7(2) . .
O5 Na4 Si1 Eu1 -27.71(13) 3_465 .
O3 Na4 Si1 Eu1 -62.6(2) 4_645 .
Eu2 Na4 Si1 Eu1 64.73(9) . .
Si2 Na4 Si1 Eu1 122.33(6) . .
O6 Na4 Si1 Eu3 -96.07(14) 2_765 3_465
O3 Na4 Si1 Eu3 177.8(3) . 3_465
O6 Na4 Si1 Eu3 81.86(11) 3_465 3_465
O4 Na4 Si1 Eu3 165.69(12) . 3_465
O1 Na4 Si1 Eu3 148.4(4) 7_755 3_465
O2 Na4 Si1 Eu3 -26.6(2) . 3_465
O5 Na4 Si1 Eu3 26.47(12) 3_465 3_465
O3 Na4 Si1 Eu3 -8.4(2) 4_645 3_465
Eu2 Na4 Si1 Eu3 118.91(9) . 3_465
Si2 Na4 Si1 Eu3 176.51(7) . 3_465
O4 Eu1 Si1 O1 138.91(10) 3_465 .
O4 Eu1 Si1 O1 -41.09(10) 7_766 .
O4 Eu1 Si1 O1 -138.91(10) 8_576 .
O4 Eu1 Si1 O1 41.09(10) 4_655 .
O1 Eu1 Si1 O1 180.0 5_676 .
Eu2 Eu1 Si1 O1 180.0 3_465 .
Na2 Eu1 Si1 O1 180.0 3_465 .
Na2 Eu1 Si1 O1 0.0 7_766 .
Eu2 Eu1 Si1 O1 0.0 7_766 .
Si1 Eu1 Si1 O1 0.0 5_676 .
O4 Eu1 Si1 O2 -41.09(10) 3_465 .
O4 Eu1 Si1 O2 138.91(10) 7_766 .
O4 Eu1 Si1 O2 41.09(10) 8_576 .
O4 Eu1 Si1 O2 -138.91(10) 4_655 .
O1 Eu1 Si1 O2 180.0 . .
O1 Eu1 Si1 O2 0.0 5_676 .
Eu2 Eu1 Si1 O2 0.0 3_465 .
Na2 Eu1 Si1 O2 0.0 3_465 .
Na2 Eu1 Si1 O2 180.0 7_766 .
Eu2 Eu1 Si1 O2 180.0 7_766 .
Si1 Eu1 Si1 O2 180(100) 5_676 .
O4 Eu1 Si1 O3 -150.1(2) 3_465 6_556
O4 Eu1 Si1 O3 29.9(2) 7_766 6_556
O4 Eu1 Si1 O3 -67.9(2) 8_576 6_556
O4 Eu1 Si1 O3 112.1(2) 4_655 6_556
O1 Eu1 Si1 O3 71.0(2) . 6_556
O1 Eu1 Si1 O3 -109.0(2) 5_676 6_556
Eu2 Eu1 Si1 O3 -109.0(2) 3_465 6_556
Na2 Eu1 Si1 O3 -109.0(2) 3_465 6_556
Na2 Eu1 Si1 O3 71.0(2) 7_766 6_556
Eu2 Eu1 Si1 O3 71.0(2) 7_766 6_556
Si1 Eu1 Si1 O3 71(100) 5_676 6_556
O4 Eu1 Si1 O3 67.9(2) 3_465 .
O4 Eu1 Si1 O3 -112.1(2) 7_766 .
O4 Eu1 Si1 O3 150.1(2) 8_576 .
O4 Eu1 Si1 O3 -29.9(2) 4_655 .
O1 Eu1 Si1 O3 -71.0(2) . .
O1 Eu1 Si1 O3 109.0(2) 5_676 .
Eu2 Eu1 Si1 O3 109.0(2) 3_465 .
Na2 Eu1 Si1 O3 109.0(2) 3_465 .
Na2 Eu1 Si1 O3 -71.0(2) 7_766 .
Eu2 Eu1 Si1 O3 -71.0(2) 7_766 .
Si1 Eu1 Si1 O3 -71(100) 5_676 .
O4 Eu1 Si1 Na1 -41.09(10) 3_465 3_565
O4 Eu1 Si1 Na1 138.91(10) 7_766 3_565
O4 Eu1 Si1 Na1 41.09(10) 8_576 3_565
O4 Eu1 Si1 Na1 -138.91(10) 4_655 3_565
O1 Eu1 Si1 Na1 180.0 . 3_565
O1 Eu1 Si1 Na1 0.0 5_676 3_565
Eu2 Eu1 Si1 Na1 0.0 3_465 3_565
Na2 Eu1 Si1 Na1 0.0 3_465 3_565
Na2 Eu1 Si1 Na1 180.0 7_766 3_565
Eu2 Eu1 Si1 Na1 180.0 7_766 3_565
Si1 Eu1 Si1 Na1 180.0 5_676 3_565
O4 Eu1 Si1 Na4 16.62(12) 3_465 .
O4 Eu1 Si1 Na4 -163.38(12) 7_766 .
O4 Eu1 Si1 Na4 98.80(12) 8_576 .
O4 Eu1 Si1 Na4 -81.20(12) 4_655 .
O1 Eu1 Si1 Na4 -122.29(6) . .
O1 Eu1 Si1 Na4 57.71(6) 5_676 .
Eu2 Eu1 Si1 Na4 57.71(6) 3_465 .
Na2 Eu1 Si1 Na4 57.71(6) 3_465 .
Na2 Eu1 Si1 Na4 -122.29(6) 7_766 .
Eu2 Eu1 Si1 Na4 -122.29(6) 7_766 .
Si1 Eu1 Si1 Na4 -122(100) 5_676 .
O4 Eu1 Si1 Na4 -98.80(12) 3_465 6_556
O4 Eu1 Si1 Na4 81.20(12) 7_766 6_556
O4 Eu1 Si1 Na4 -16.62(12) 8_576 6_556
O4 Eu1 Si1 Na4 163.38(12) 4_655 6_556
O1 Eu1 Si1 Na4 122.29(6) . 6_556
O1 Eu1 Si1 Na4 -57.71(6) 5_676 6_556
Eu2 Eu1 Si1 Na4 -57.71(6) 3_465 6_556
Na2 Eu1 Si1 Na4 -57.71(6) 3_465 6_556
Na2 Eu1 Si1 Na4 122.29(6) 7_766 6_556
Eu2 Eu1 Si1 Na4 122.29(6) 7_766 6_556
Si1 Eu1 Si1 Na4 122(100) 5_676 6_556
O4 Eu1 Si1 Na4 -160.39(12) 3_465 7_766
O4 Eu1 Si1 Na4 19.61(12) 7_766 7_766
O4 Eu1 Si1 Na4 -78.21(11) 8_576 7_766
O4 Eu1 Si1 Na4 101.79(11) 4_655 7_766
O1 Eu1 Si1 Na4 60.70(5) . 7_766
O1 Eu1 Si1 Na4 -119.30(5) 5_676 7_766
Eu2 Eu1 Si1 Na4 -119.30(5) 3_465 7_766
Na2 Eu1 Si1 Na4 -119.30(5) 3_465 7_766
Na2 Eu1 Si1 Na4 60.70(5) 7_766 7_766
Eu2 Eu1 Si1 Na4 60.70(5) 7_766 7_766
Si1 Eu1 Si1 Na4 61(100) 5_676 7_766
O4 Eu1 Si1 Na4 78.21(11) 3_465 4_655
O4 Eu1 Si1 Na4 -101.79(11) 7_766 4_655
O4 Eu1 Si1 Na4 160.39(12) 8_576 4_655
O4 Eu1 Si1 Na4 -19.61(12) 4_655 4_655
O1 Eu1 Si1 Na4 -60.70(5) . 4_655
O1 Eu1 Si1 Na4 119.30(5) 5_676 4_655
Eu2 Eu1 Si1 Na4 119.30(5) 3_465 4_655
Na2 Eu1 Si1 Na4 119.30(5) 3_465 4_655
Na2 Eu1 Si1 Na4 -60.70(5) 7_766 4_655
Eu2 Eu1 Si1 Na4 -60.70(5) 7_766 4_655
Si1 Eu1 Si1 Na4 -61(100) 5_676 4_655
O4 Eu1 Si1 Eu3 -41.09(10) 3_465 3_465
O4 Eu1 Si1 Eu3 138.91(10) 7_766 3_465
O4 Eu1 Si1 Eu3 41.09(10) 8_576 3_465
O4 Eu1 Si1 Eu3 -138.91(10) 4_655 3_465
O1 Eu1 Si1 Eu3 180.0 . 3_465
O1 Eu1 Si1 Eu3 0.0 5_676 3_465
Eu2 Eu1 Si1 Eu3 0.0 3_465 3_465
Na2 Eu1 Si1 Eu3 0.0 3_465 3_465
Na2 Eu1 Si1 Eu3 180.0 7_766 3_465
Eu2 Eu1 Si1 Eu3 180.0 7_766 3_465
Si1 Eu1 Si1 Eu3 180.0 5_676 3_465
O6 Na4 Si2 O6 1.30(18) 2_765 .
O3 Na4 Si2 O6 95.2(3) . .
O6 Na4 Si2 O6 177.96(15) 3_465 .
O4 Na4 Si2 O6 -105.5(3) . .
O1 Na4 Si2 O6 -94.3(3) 7_755 .
O2 Na4 Si2 O6 85.3(2) . .
O5 Na4 Si2 O6 156.2(4) 3_465 .
O3 Na4 Si2 O6 -77.4(4) 4_645 .
Eu2 Na4 Si2 O6 -137.9(2) . .
Si1 Na4 Si2 O6 96.5(2) . .
O6 Na4 Si2 O4 106.8(2) 2_765 .
O3 Na4 Si2 O4 -159.3(3) . .
O6 Na4 Si2 O4 -76.6(2) 3_465 .
O1 Na4 Si2 O4 11.1(2) 7_755 .
O2 Na4 Si2 O4 -169.3(2) . .
O5 Na4 Si2 O4 -98.3(4) 3_465 .
O3 Na4 Si2 O4 28.1(3) 4_645 .
Eu2 Na4 Si2 O4 -32.42(18) . .
Si1 Na4 Si2 O4 -158.0(2) . .
O6 Na4 Si2 O5 -172.4(4) 2_765 .
O3 Na4 Si2 O5 -78.4(5) . .
O6 Na4 Si2 O5 4.3(5) 3_465 .
O4 Na4 Si2 O5 80.9(5) . .
O1 Na4 Si2 O5 92.0(4) 7_755 .
O2 Na4 Si2 O5 -88.4(5) . .
O5 Na4 Si2 O5 -17.4(8) 3_465 .
O3 Na4 Si2 O5 109.0(5) 4_645 .
Eu2 Na4 Si2 O5 48.5(4) . .
Si1 Na4 Si2 O5 -77.1(4) . .
O6 Na4 Si2 O3 -93.9(3) 2_765 .
O6 Na4 Si2 O3 82.7(3) 3_465 .
O4 Na4 Si2 O3 159.3(3) . .
O1 Na4 Si2 O3 170.5(3) 7_755 .
O2 Na4 Si2 O3 -9.9(3) . .
O5 Na4 Si2 O3 61.0(5) 3_465 .
O3 Na4 Si2 O3 -172.6(4) 4_645 .
Eu2 Na4 Si2 O3 126.9(3) . .
Si1 Na4 Si2 O3 1.3(3) . .
O6 Na4 Si2 Na1 -34.10(13) 2_765 3_565
O3 Na4 Si2 Na1 59.8(3) . 3_565
O6 Na4 Si2 Na1 142.57(12) 3_465 3_565
O4 Na4 Si2 Na1 -140.8(2) . 3_565
O1 Na4 Si2 Na1 -129.70(14) 7_755 3_565
O2 Na4 Si2 Na1 49.89(12) . 3_565
O5 Na4 Si2 Na1 120.8(4) 3_465 3_565
O3 Na4 Si2 Na1 -112.7(3) 4_645 3_565
Eu2 Na4 Si2 Na1 -173.27(6) . 3_565
Si1 Na4 Si2 Na1 61.12(5) . 3_565
O6 Na4 Si2 Na4 58.7(3) 2_765 3_565
O3 Na4 Si2 Na4 152.6(4) . 3_565
O6 Na4 Si2 Na4 -124.6(3) 3_465 3_565
O4 Na4 Si2 Na4 -48.0(3) . 3_565
O1 Na4 Si2 Na4 -36.9(3) 7_755 3_565
O2 Na4 Si2 Na4 142.7(3) . 3_565
O5 Na4 Si2 Na4 -146.4(4) 3_465 3_565
O3 Na4 Si2 Na4 -19.9(4) 4_645 3_565
Eu2 Na4 Si2 Na4 -80.5(3) . 3_565
Si1 Na4 Si2 Na4 153.9(3) . 3_565
O6 Na4 Si2 Na4 -162.59(18) 2_765 4_655
O3 Na4 Si2 Na4 -68.7(3) . 4_655
O6 Na4 Si2 Na4 14.07(10) 3_465 4_655
O4 Na4 Si2 Na4 90.7(2) . 4_655
O1 Na4 Si2 Na4 101.81(16) 7_755 4_655
O2 Na4 Si2 Na4 -78.60(14) . 4_655
O5 Na4 Si2 Na4 -7.7(4) 3_465 4_655
O3 Na4 Si2 Na4 118.8(3) 4_645 4_655
Eu2 Na4 Si2 Na4 58.24(6) . 4_655
Si1 Na4 Si2 Na4 -67.38(8) . 4_655
O6 Na4 Si2 Eu3 132.23(14) 2_765 .
O3 Na4 Si2 Eu3 -133.8(3) . .
O6 Na4 Si2 Eu3 -51.11(12) 3_465 .
O4 Na4 Si2 Eu3 25.48(18) . .
O1 Na4 Si2 Eu3 36.63(14) 7_755 .
O2 Na4 Si2 Eu3 -143.78(13) . .
O5 Na4 Si2 Eu3 -72.9(4) 3_465 .
O3 Na4 Si2 Eu3 53.6(3) 4_645 .
Eu2 Na4 Si2 Eu3 -6.94(5) . .
Si1 Na4 Si2 Eu3 -132.56(7) . .
O6 Na4 Si2 Eu1 78.19(13) 2_765 3_565
O3 Na4 Si2 Eu1 172.1(3) . 3_565
O6 Na4 Si2 Eu1 -105.15(12) 3_465 3_565
O4 Na4 Si2 Eu1 -28.57(18) . 3_565
O1 Na4 Si2 Eu1 -17.42(13) 7_755 3_565
O2 Na4 Si2 Eu1 162.18(14) . 3_565
O5 Na4 Si2 Eu1 -126.9(4) 3_465 3_565
O3 Na4 Si2 Eu1 -0.5(3) 4_645 3_565
Eu2 Na4 Si2 Eu1 -60.99(4) . 3_565
Si1 Na4 Si2 Eu1 173.40(7) . 3_565
O6 Na4 Si2 Eu2 -25.95(16) 2_765 3_565
O3 Na4 Si2 Eu2 68.0(3) . 3_565
O6 Na4 Si2 Eu2 150.72(12) 3_465 3_565
O4 Na4 Si2 Eu2 -132.7(2) . 3_565
O1 Na4 Si2 Eu2 -121.55(15) 7_755 3_565
O2 Na4 Si2 Eu2 58.04(14) . 3_565
O5 Na4 Si2 Eu2 129.0(4) 3_465 3_565
O3 Na4 Si2 Eu2 -104.6(3) 4_645 3_565
Eu2 Na4 Si2 Eu2 -165.12(7) . 3_565
Si1 Na4 Si2 Eu2 69.27(8) . 3_565
O2 Eu3 Si2 O6 2.6(2) 3_565 .
O2 Eu3 Si2 O6 -177.4(2) 7_765 .
O4 Eu3 Si2 O6 93.1(2) 6 .
O4 Eu3 Si2 O6 -86.9(2) 2_775 .
O4 Eu3 Si2 O6 105.4(3) . .
O4 Eu3 Si2 O6 -74.6(3) 5_775 .
O5 Eu3 Si2 O6 82.1(2) 5_775 .
O5 Eu3 Si2 O6 -97.9(2) . .
Eu2 Eu3 Si2 O6 138.8(2) . .
Eu2 Eu3 Si2 O6 -41.2(2) 5_775 .
Si2 Eu3 Si2 O6 82.1(2) 6 .
Si2 Eu3 Si2 O6 -97.9(2) 2_775 .
O2 Eu3 Si2 O4 -102.8(2) 3_565 .
O2 Eu3 Si2 O4 77.2(2) 7_765 .
O4 Eu3 Si2 O4 -12.37(12) 6 .
O4 Eu3 Si2 O4 167.63(12) 2_775 .
O4 Eu3 Si2 O4 180.0 5_775 .
O5 Eu3 Si2 O4 -23.3(2) 5_775 .
O5 Eu3 Si2 O4 156.7(2) . .
Eu2 Eu3 Si2 O4 33.34(19) . .
Eu2 Eu3 Si2 O4 -146.66(19) 5_775 .
Si2 Eu3 Si2 O4 -23.3(2) 6 .
Si2 Eu3 Si2 O4 156.7(2) 2_775 .
O2 Eu3 Si2 O5 100.50(13) 3_565 .
O2 Eu3 Si2 O5 -79.50(13) 7_765 .
O4 Eu3 Si2 O5 -169.07(10) 6 .
O4 Eu3 Si2 O5 10.93(10) 2_775 .
O4 Eu3 Si2 O5 -156.7(2) . .
O4 Eu3 Si2 O5 23.3(2) 5_775 .
O5 Eu3 Si2 O5 180.000(1) 5_775 .
Eu2 Eu3 Si2 O5 -123.36(5) . .
Eu2 Eu3 Si2 O5 56.64(5) 5_775 .
Si2 Eu3 Si2 O5 180.000(1) 6 .
Si2 Eu3 Si2 O5 0.000(1) 2_775 .
O2 Eu3 Si2 O3 -180.0(3) 3_565 .
O2 Eu3 Si2 O3 0.0(3) 7_765 .
O4 Eu3 Si2 O3 -89.5(3) 6 .
O4 Eu3 Si2 O3 90.5(3) 2_775 .
O4 Eu3 Si2 O3 -77.2(3) . .
O4 Eu3 Si2 O3 102.8(3) 5_775 .
O5 Eu3 Si2 O3 -100.5(2) 5_775 .
O5 Eu3 Si2 O3 79.5(2) . .
Eu2 Eu3 Si2 O3 -43.8(2) . .
Eu2 Eu3 Si2 O3 136.2(2) 5_775 .
Si2 Eu3 Si2 O3 -100.5(2) 6 .
Si2 Eu3 Si2 O3 79.5(2) 2_775 .
O2 Eu3 Si2 Na4 -129.16(13) 3_565 .
O2 Eu3 Si2 Na4 50.84(13) 7_765 .
O4 Eu3 Si2 Na4 -38.73(11) 6 .
O4 Eu3 Si2 Na4 141.27(11) 2_775 .
O4 Eu3 Si2 Na4 -26.36(19) . .
O4 Eu3 Si2 Na4 153.64(19) 5_775 .
O5 Eu3 Si2 Na4 -49.66(8) 5_775 .
O5 Eu3 Si2 Na4 130.34(8) . .
Eu2 Eu3 Si2 Na4 6.98(5) . .
Eu2 Eu3 Si2 Na4 -173.02(5) 5_775 .
Si2 Eu3 Si2 Na4 -49.66(8) 6 .
Si2 Eu3 Si2 Na4 130.34(8) 2_775 .
O2 Eu3 Si2 Na1 -62.8(2) 3_565 3_565
O2 Eu3 Si2 Na1 117.2(2) 7_765 3_565
O4 Eu3 Si2 Na1 27.7(2) 6 3_565
O4 Eu3 Si2 Na1 -152.3(2) 2_775 3_565
O4 Eu3 Si2 Na1 40.0(2) . 3_565
O4 Eu3 Si2 Na1 -140.0(2) 5_775 3_565
O5 Eu3 Si2 Na1 16.7(2) 5_775 3_565
O5 Eu3 Si2 Na1 -163.3(2) . 3_565
Eu2 Eu3 Si2 Na1 73.37(18) . 3_565
Eu2 Eu3 Si2 Na1 -106.63(18) 5_775 3_565
Si2 Eu3 Si2 Na1 16.7(2) 6 3_565
Si2 Eu3 Si2 Na1 -163.3(2) 2_775 3_565
O2 Eu3 Si2 Na4 34.77(14) 3_565 3_565
O2 Eu3 Si2 Na4 -145.23(14) 7_765 3_565
O4 Eu3 Si2 Na4 125.20(11) 6 3_565
O4 Eu3 Si2 Na4 -54.80(11) 2_775 3_565
O4 Eu3 Si2 Na4 137.6(2) . 3_565
O4 Eu3 Si2 Na4 -42.4(2) 5_775 3_565
O5 Eu3 Si2 Na4 114.27(6) 5_775 3_565
O5 Eu3 Si2 Na4 -65.73(6) . 3_565
Eu2 Eu3 Si2 Na4 170.91(7) . 3_565
Eu2 Eu3 Si2 Na4 -9.09(7) 5_775 3_565
Si2 Eu3 Si2 Na4 114.27(6) 6 3_565
Si2 Eu3 Si2 Na4 -65.73(6) 2_775 3_565
O2 Eu3 Si2 Na4 165.60(13) 3_565 4_655
O2 Eu3 Si2 Na4 -14.40(13) 7_765 4_655
O4 Eu3 Si2 Na4 -103.97(10) 6 4_655
O4 Eu3 Si2 Na4 76.03(10) 2_775 4_655
O4 Eu3 Si2 Na4 -91.6(2) . 4_655
O4 Eu3 Si2 Na4 88.4(2) 5_775 4_655
O5 Eu3 Si2 Na4 -114.91(6) 5_775 4_655
O5 Eu3 Si2 Na4 65.09(6) . 4_655
Eu2 Eu3 Si2 Na4 -58.26(5) . 4_655
Eu2 Eu3 Si2 Na4 121.74(5) 5_775 4_655
Si2 Eu3 Si2 Na4 -114.91(6) 6 4_655
Si2 Eu3 Si2 Na4 65.09(6) 2_775 4_655
O2 Eu3 Si2 Eu1 -75.60(12) 3_565 3_565
O2 Eu3 Si2 Eu1 104.40(12) 7_765 3_565
O4 Eu3 Si2 Eu1 14.83(9) 6 3_565
O4 Eu3 Si2 Eu1 -165.17(9) 2_775 3_565
O4 Eu3 Si2 Eu1 27.20(19) . 3_565
O4 Eu3 Si2 Eu1 -152.80(19) 5_775 3_565
O5 Eu3 Si2 Eu1 3.89(5) 5_775 3_565
O5 Eu3 Si2 Eu1 -176.11(5) . 3_565
Eu2 Eu3 Si2 Eu1 60.54(3) . 3_565
Eu2 Eu3 Si2 Eu1 -119.46(3) 5_775 3_565
Si2 Eu3 Si2 Eu1 3.89(5) 6 3_565
Si2 Eu3 Si2 Eu1 -176.11(5) 2_775 3_565
O2 Eu3 Si2 Eu2 28.91(14) 3_565 3_565
O2 Eu3 Si2 Eu2 -151.09(14) 7_765 3_565
O4 Eu3 Si2 Eu2 119.34(11) 6 3_565
O4 Eu3 Si2 Eu2 -60.66(11) 2_775 3_565
O4 Eu3 Si2 Eu2 131.7(2) . 3_565
O4 Eu3 Si2 Eu2 -48.3(2) 5_775 3_565
O5 Eu3 Si2 Eu2 108.41(6) 5_775 3_565
O5 Eu3 Si2 Eu2 -71.59(6) . 3_565
Eu2 Eu3 Si2 Eu2 165.05(7) . 3_565
Eu2 Eu3 Si2 Eu2 -14.95(7) 5_775 3_565
Si2 Eu3 Si2 Eu2 108.41(6) 6 3_565
Si2 Eu3 Si2 Eu2 -71.59(6) 2_775 3_565
O2 Si1 O1 Eu1 0.0 . .
O3 Si1 O1 Eu1 -122.5(2) 6_556 .
O3 Si1 O1 Eu1 122.5(2) . .
Na1 Si1 O1 Eu1 180.0 3_565 .
Na4 Si1 O1 Eu1 66.46(12) . .
Na4 Si1 O1 Eu1 -66.46(12) 6_556 .
Na4 Si1 O1 Eu1 -102.64(16) 7_766 .
Na4 Si1 O1 Eu1 102.64(16) 4_655 .
Eu3 Si1 O1 Eu1 0.0 3_465 .
O2 Si1 O1 Na2 180.0 . 7_766
O3 Si1 O1 Na2 57.5(2) 6_556 7_766
O3 Si1 O1 Na2 -57.5(2) . 7_766
Na1 Si1 O1 Na2 0.0 3_565 7_766
Na4 Si1 O1 Na2 -113.54(12) . 7_766
Na4 Si1 O1 Na2 113.54(12) 6_556 7_766
Na4 Si1 O1 Na2 77.36(16) 7_766 7_766
Na4 Si1 O1 Na2 -77.36(16) 4_655 7_766
Eu1 Si1 O1 Na2 180.0 . 7_766
Eu3 Si1 O1 Na2 180.0 3_465 7_766
O2 Si1 O1 Eu2 180.0 . 7_766
O3 Si1 O1 Eu2 57.5(2) 6_556 7_766
O3 Si1 O1 Eu2 -57.5(2) . 7_766
Na1 Si1 O1 Eu2 0.0 3_565 7_766
Na4 Si1 O1 Eu2 -113.54(12) . 7_766
Na4 Si1 O1 Eu2 113.54(12) 6_556 7_766
Na4 Si1 O1 Eu2 77.36(16) 7_766 7_766
Na4 Si1 O1 Eu2 -77.36(16) 4_655 7_766
Eu1 Si1 O1 Eu2 180.0 . 7_766
Eu3 Si1 O1 Eu2 180.0 3_465 7_766
O2 Si1 O1 Na4 102.64(16) . 7_766
O3 Si1 O1 Na4 -19.9(3) 6_556 7_766
O3 Si1 O1 Na4 -134.9(2) . 7_766
Na1 Si1 O1 Na4 -77.36(16) 3_565 7_766
Na4 Si1 O1 Na4 169.10(10) . 7_766
Na4 Si1 O1 Na4 36.2(3) 6_556 7_766
Na4 Si1 O1 Na4 -154.7(3) 4_655 7_766
Eu1 Si1 O1 Na4 102.64(16) . 7_766
Eu3 Si1 O1 Na4 102.64(16) 3_465 7_766
O2 Si1 O1 Na4 -102.64(16) . 4_655
O3 Si1 O1 Na4 134.9(2) 6_556 4_655
O3 Si1 O1 Na4 19.9(3) . 4_655
Na1 Si1 O1 Na4 77.36(16) 3_565 4_655
Na4 Si1 O1 Na4 -36.2(3) . 4_655
Na4 Si1 O1 Na4 -169.10(10) 6_556 4_655
Na4 Si1 O1 Na4 154.7(3) 7_766 4_655
Eu1 Si1 O1 Na4 -102.64(16) . 4_655
Eu3 Si1 O1 Na4 -102.64(16) 3_465 4_655
O4 Eu1 O1 Si1 -41.21(11) 3_465 .
O4 Eu1 O1 Si1 138.79(11) 7_766 .
O4 Eu1 O1 Si1 41.21(11) 8_576 .
O4 Eu1 O1 Si1 -138.79(11) 4_655 .
O1 Eu1 O1 Si1 180(100) 5_676 .
Eu2 Eu1 O1 Si1 0.0 3_465 .
Na2 Eu1 O1 Si1 0.0 3_465 .
Na2 Eu1 O1 Si1 180.0 7_766 .
Eu2 Eu1 O1 Si1 180.0 7_766 .
Si1 Eu1 O1 Si1 180.0 5_676 .
O4 Eu1 O1 Na2 138.79(11) 3_465 7_766
O4 Eu1 O1 Na2 -41.21(11) 7_766 7_766
O4 Eu1 O1 Na2 -138.79(11) 8_576 7_766
O4 Eu1 O1 Na2 41.21(11) 4_655 7_766
O1 Eu1 O1 Na2 0.0 5_676 7_766
Eu2 Eu1 O1 Na2 180.0 3_465 7_766
Na2 Eu1 O1 Na2 180.0 3_465 7_766
Eu2 Eu1 O1 Na2 0.0 7_766 7_766
Si1 Eu1 O1 Na2 180.0 . 7_766
Si1 Eu1 O1 Na2 0.0 5_676 7_766
O4 Eu1 O1 Eu2 138.79(11) 3_465 7_766
O4 Eu1 O1 Eu2 -41.21(11) 7_766 7_766
O4 Eu1 O1 Eu2 -138.79(11) 8_576 7_766
O4 Eu1 O1 Eu2 41.21(11) 4_655 7_766
O1 Eu1 O1 Eu2 0.0 5_676 7_766
Eu2 Eu1 O1 Eu2 180.0 3_465 7_766
Na2 Eu1 O1 Eu2 180.0 3_465 7_766
Na2 Eu1 O1 Eu2 0.0 7_766 7_766
Si1 Eu1 O1 Eu2 180.0 . 7_766
Si1 Eu1 O1 Eu2 0.0 5_676 7_766
O4 Eu1 O1 Na4 -145.84(17) 3_465 7_766
O4 Eu1 O1 Na4 34.16(17) 7_766 7_766
O4 Eu1 O1 Na4 -63.42(18) 8_576 7_766
O4 Eu1 O1 Na4 116.58(18) 4_655 7_766
O1 Eu1 O1 Na4 75(100) 5_676 7_766
Eu2 Eu1 O1 Na4 -104.63(14) 3_465 7_766
Na2 Eu1 O1 Na4 -104.63(14) 3_465 7_766
Na2 Eu1 O1 Na4 75.37(14) 7_766 7_766
Eu2 Eu1 O1 Na4 75.37(14) 7_766 7_766
Si1 Eu1 O1 Na4 -104.63(14) . 7_766
Si1 Eu1 O1 Na4 75.37(14) 5_676 7_766
O4 Eu1 O1 Na4 63.42(18) 3_465 4_655
O4 Eu1 O1 Na4 -116.58(18) 7_766 4_655
O4 Eu1 O1 Na4 145.84(17) 8_576 4_655
O4 Eu1 O1 Na4 -34.16(17) 4_655 4_655
O1 Eu1 O1 Na4 -75(100) 5_676 4_655
Eu2 Eu1 O1 Na4 104.63(14) 3_465 4_655
Na2 Eu1 O1 Na4 104.63(14) 3_465 4_655
Na2 Eu1 O1 Na4 -75.37(14) 7_766 4_655
Eu2 Eu1 O1 Na4 -75.37(14) 7_766 4_655
Si1 Eu1 O1 Na4 104.63(14) . 4_655
Si1 Eu1 O1 Na4 -75.37(14) 5_676 4_655
O1 Si1 O2 Na3 0.0 . 3_465
O3 Si1 O2 Na3 124.5(2) 6_556 3_465
O3 Si1 O2 Na3 -124.5(2) . 3_465
Na1 Si1 O2 Na3 180.0 3_565 3_465
Na4 Si1 O2 Na3 -104.83(13) . 3_465
Na4 Si1 O2 Na3 104.83(13) 6_556 3_465
Na4 Si1 O2 Na3 60.17(12) 7_766 3_465
Na4 Si1 O2 Na3 -60.17(12) 4_655 3_465
Eu1 Si1 O2 Na3 0.0 . 3_465
Eu3 Si1 O2 Na3 0.0 3_465 3_465
O1 Si1 O2 Eu3 0.0 . 3_465
O3 Si1 O2 Eu3 124.5(2) 6_556 3_465
O3 Si1 O2 Eu3 -124.5(2) . 3_465
Na1 Si1 O2 Eu3 180.0 3_565 3_465
Na4 Si1 O2 Eu3 -104.83(13) . 3_465
Na4 Si1 O2 Eu3 104.83(13) 6_556 3_465
Na4 Si1 O2 Eu3 60.17(12) 7_766 3_465
Na4 Si1 O2 Eu3 -60.17(12) 4_655 3_465
Eu1 Si1 O2 Eu3 0.0 . 3_465
O1 Si1 O2 Na2 180.0 . 7_756
O3 Si1 O2 Na2 -55.5(2) 6_556 7_756
O3 Si1 O2 Na2 55.5(2) . 7_756
Na1 Si1 O2 Na2 0.0 3_565 7_756
Na4 Si1 O2 Na2 75.17(13) . 7_756
Na4 Si1 O2 Na2 -75.17(13) 6_556 7_756
Na4 Si1 O2 Na2 -119.83(12) 7_766 7_756
Na4 Si1 O2 Na2 119.83(12) 4_655 7_756
Eu1 Si1 O2 Na2 180.0 . 7_756
Eu3 Si1 O2 Na2 180.0 3_465 7_756
O1 Si1 O2 Eu2 180.0 . 7_756
O3 Si1 O2 Eu2 -55.5(2) 6_556 7_756
O3 Si1 O2 Eu2 55.5(2) . 7_756
Na1 Si1 O2 Eu2 0.0 3_565 7_756
Na4 Si1 O2 Eu2 75.17(13) . 7_756
Na4 Si1 O2 Eu2 -75.17(13) 6_556 7_756
Na4 Si1 O2 Eu2 -119.83(12) 7_766 7_756
Na4 Si1 O2 Eu2 119.83(12) 4_655 7_756
Eu1 Si1 O2 Eu2 180.0 . 7_756
Eu3 Si1 O2 Eu2 180.0 3_465 7_756
O1 Si1 O2 Na4 -104.83(13) . 6_556
O3 Si1 O2 Na4 19.7(3) 6_556 6_556
O3 Si1 O2 Na4 130.6(3) . 6_556
Na1 Si1 O2 Na4 75.17(13) 3_565 6_556
Na4 Si1 O2 Na4 150.3(3) . 6_556
Na4 Si1 O2 Na4 -44.7(2) 7_766 6_556
Na4 Si1 O2 Na4 -165.00(10) 4_655 6_556
Eu1 Si1 O2 Na4 -104.83(13) . 6_556
Eu3 Si1 O2 Na4 -104.83(13) 3_465 6_556
O1 Si1 O2 Na4 104.83(13) . .
O3 Si1 O2 Na4 -130.6(3) 6_556 .
O3 Si1 O2 Na4 -19.7(3) . .
Na1 Si1 O2 Na4 -75.17(13) 3_565 .
Na4 Si1 O2 Na4 -150.3(3) 6_556 .
Na4 Si1 O2 Na4 165.00(10) 7_766 .
Na4 Si1 O2 Na4 44.7(2) 4_655 .
Eu1 Si1 O2 Na4 104.83(13) . .
Eu3 Si1 O2 Na4 104.83(13) 3_465 .
O6 Na4 O2 Si1 110.1(3) 2_765 .
O3 Na4 O2 Si1 14.0(2) . .
O6 Na4 O2 Si1 -70.5(2) 3_465 .
O4 Na4 O2 Si1 13.9(3) . .
O1 Na4 O2 Si1 -163.4(14) 7_755 .
O5 Na4 O2 Si1 -126.8(2) 3_465 .
O3 Na4 O2 Si1 -168.7(2) 4_645 .
Eu2 Na4 O2 Si1 -47.5(3) . .
Si2 Na4 O2 Si1 20.0(2) . .
O6 Na4 O2 Na3 -111.3(2) 2_765 3_465
O3 Na4 O2 Na3 152.6(3) . 3_465
O6 Na4 O2 Na3 68.16(19) 3_465 3_465
O4 Na4 O2 Na3 152.50(17) . 3_465
O1 Na4 O2 Na3 -24.7(16) 7_755 3_465
O5 Na4 O2 Na3 11.80(15) 3_465 3_465
O3 Na4 O2 Na3 -30.1(3) 4_645 3_465
Eu2 Na4 O2 Na3 91.2(2) . 3_465
Si2 Na4 O2 Na3 158.58(17) . 3_465
Si1 Na4 O2 Na3 138.6(3) . 3_465
O6 Na4 O2 Eu3 -111.3(2) 2_765 3_465
O3 Na4 O2 Eu3 152.6(3) . 3_465
O6 Na4 O2 Eu3 68.16(19) 3_465 3_465
O4 Na4 O2 Eu3 152.50(17) . 3_465
O1 Na4 O2 Eu3 -24.7(16) 7_755 3_465
O5 Na4 O2 Eu3 11.80(15) 3_465 3_465
O3 Na4 O2 Eu3 -30.1(3) 4_645 3_465
Eu2 Na4 O2 Eu3 91.2(2) . 3_465
Si2 Na4 O2 Eu3 158.58(17) . 3_465
Si1 Na4 O2 Eu3 138.6(3) . 3_465
O6 Na4 O2 Na2 -28.40(17) 2_765 7_756
O3 Na4 O2 Na2 -124.5(2) . 7_756
O6 Na4 O2 Na2 151.04(16) 3_465 7_756
O4 Na4 O2 Na2 -124.62(17) . 7_756
O1 Na4 O2 Na2 58.1(16) 7_755 7_756
O5 Na4 O2 Na2 94.67(13) 3_465 7_756
O3 Na4 O2 Na2 52.8(2) 4_645 7_756
Eu2 Na4 O2 Na2 174.03(14) . 7_756
Si2 Na4 O2 Na2 -118.54(13) . 7_756
Si1 Na4 O2 Na2 -138.5(3) . 7_756
O6 Na4 O2 Eu2 -28.40(17) 2_765 7_756
O3 Na4 O2 Eu2 -124.5(2) . 7_756
O6 Na4 O2 Eu2 151.04(16) 3_465 7_756
O4 Na4 O2 Eu2 -124.62(17) . 7_756
O1 Na4 O2 Eu2 58.1(16) 7_755 7_756
O5 Na4 O2 Eu2 94.67(13) 3_465 7_756
O3 Na4 O2 Eu2 52.8(2) 4_645 7_756
Eu2 Na4 O2 Eu2 174.03(14) . 7_756
Si2 Na4 O2 Eu2 -118.54(13) . 7_756
Si1 Na4 O2 Eu2 -138.5(3) . 7_756
O6 Na4 O2 Na4 15.1(5) 2_765 6_556
O3 Na4 O2 Na4 -81.0(5) . 6_556
O6 Na4 O2 Na4 -165.5(4) 3_465 6_556
O4 Na4 O2 Na4 -81.1(5) . 6_556
O1 Na4 O2 Na4 101.6(15) 7_755 6_556
O5 Na4 O2 Na4 138.1(5) 3_465 6_556
O3 Na4 O2 Na4 96.3(5) 4_645 6_556
Eu2 Na4 O2 Na4 -142.5(4) . 6_556
Si2 Na4 O2 Na4 -75.1(5) . 6_556
Si1 Na4 O2 Na4 -95.0(5) . 6_556
O1 Si1 O3 Si2 65.2(16) . .
O2 Si1 O3 Si2 -166.5(15) . .
O3 Si1 O3 Si2 -53.8(17) 6_556 .
Na1 Si1 O3 Si2 -96.9(15) 3_565 .
Na4 Si1 O3 Si2 171.9(17) . .
Na4 Si1 O3 Si2 -103.7(15) 6_556 .
Na4 Si1 O3 Si2 7.2(18) 7_766 .
Na4 Si1 O3 Si2 83.5(15) 4_655 .
Eu1 Si1 O3 Si2 94.2(15) . .
Eu3 Si1 O3 Si2 169.6(14) 3_465 .
O1 Si1 O3 Na4 -106.7(3) . .
O2 Si1 O3 Na4 21.7(3) . .
O3 Si1 O3 Na4 134.33(18) 6_556 .
Na1 Si1 O3 Na4 91.28(19) 3_565 .
Na4 Si1 O3 Na4 84.4(3) 6_556 .
Na4 Si1 O3 Na4 -164.66(17) 7_766 .
Na4 Si1 O3 Na4 -88.3(2) 4_655 .
Eu1 Si1 O3 Na4 -77.6(2) . .
Eu3 Si1 O3 Na4 -2.3(3) 3_465 .
O1 Si1 O3 Na1 162.0(2) . 3_565
O2 Si1 O3 Na1 -69.6(2) . 3_565
O3 Si1 O3 Na1 43.0(3) 6_556 3_565
Na4 Si1 O3 Na1 -91.28(19) . 3_565
Na4 Si1 O3 Na1 -6.9(3) 6_556 3_565
Na4 Si1 O3 Na1 104.1(3) 7_766 3_565
Na4 Si1 O3 Na1 -179.6(2) 4_655 3_565
Eu1 Si1 O3 Na1 -168.89(9) . 3_565
Eu3 Si1 O3 Na1 -93.59(17) 3_465 3_565
O1 Si1 O3 Na4 -18.3(3) . 4_655
O2 Si1 O3 Na4 110.0(2) . 4_655
O3 Si1 O3 Na4 -137.3(2) 6_556 4_655
Na1 Si1 O3 Na4 179.6(2) 3_565 4_655
Na4 Si1 O3 Na4 88.3(2) . 4_655
Na4 Si1 O3 Na4 172.74(15) 6_556 4_655
Na4 Si1 O3 Na4 -76.3(3) 7_766 4_655
Eu1 Si1 O3 Na4 10.7(2) . 4_655
Eu3 Si1 O3 Na4 86.03(16) 3_465 4_655
O6 Si2 O3 Si1 78.0(16) . .
O4 Si2 O3 Si1 -154.1(15) . .
O5 Si2 O3 Si1 -42.5(16) . .
Na4 Si2 O3 Si1 -171.9(17) . .
Na1 Si2 O3 Si1 95.9(15) 3_565 .
Na4 Si2 O3 Si1 19.8(18) 3_565 .
Na4 Si2 O3 Si1 -84.0(15) 4_655 .
Eu3 Si2 O3 Si1 -99.5(15) . .
Eu1 Si2 O3 Si1 -179.9(14) 3_565 .
Eu2 Si2 O3 Si1 57.4(15) 3_565 .
O6 Si2 O3 Na4 -110.1(2) . .
O4 Si2 O3 Na4 17.7(3) . .
O5 Si2 O3 Na4 129.3(3) . .
Na1 Si2 O3 Na4 -92.25(19) 3_565 .
Na4 Si2 O3 Na4 -168.29(18) 3_565 .
Na4 Si2 O3 Na4 87.88(19) 4_655 .
Eu3 Si2 O3 Na4 72.4(3) . .
Eu1 Si2 O3 Na4 -8.0(3) 3_565 .
Eu2 Si2 O3 Na4 -130.76(16) 3_565 .
O6 Si2 O3 Na1 -17.9(3) . 3_565
O4 Si2 O3 Na1 110.0(2) . 3_565
O5 Si2 O3 Na1 -138.4(3) . 3_565
Na4 Si2 O3 Na1 92.25(19) . 3_565
Na4 Si2 O3 Na1 -76.0(3) 3_565 3_565
Na4 Si2 O3 Na1 -179.9(2) 4_655 3_565
Eu3 Si2 O3 Na1 164.62(11) . 3_565
Eu1 Si2 O3 Na1 84.27(18) 3_565 3_565
Eu2 Si2 O3 Na1 -38.51(14) 3_565 3_565
O6 Si2 O3 Na4 162.0(2) . 4_655
O4 Si2 O3 Na4 -70.1(2) . 4_655
O5 Si2 O3 Na4 41.5(3) . 4_655
Na4 Si2 O3 Na4 -87.88(19) . 4_655
Na1 Si2 O3 Na4 179.9(2) 3_565 4_655
Na4 Si2 O3 Na4 103.8(3) 3_565 4_655
Eu3 Si2 O3 Na4 -15.5(3) . 4_655
Eu1 Si2 O3 Na4 -95.86(14) 3_565 4_655
Eu2 Si2 O3 Na4 141.36(10) 3_565 4_655
O6 Na4 O3 Si1 -95.6(3) 2_765 .
O6 Na4 O3 Si1 81.2(3) 3_465 .
O4 Na4 O3 Si1 165.9(3) . .
O1 Na4 O3 Si1 165.6(2) 7_755 .
O2 Na4 O3 Si1 -14.0(2) . .
O5 Na4 O3 Si1 35.0(4) 3_465 .
O3 Na4 O3 Si1 -40.4(18) 4_645 .
Eu2 Na4 O3 Si1 126.9(2) . .
Si2 Na4 O3 Si1 177.7(5) . .
O6 Na4 O3 Si2 86.6(3) 2_765 .
O6 Na4 O3 Si2 -96.5(3) 3_465 .
O4 Na4 O3 Si2 -11.8(2) . .
O1 Na4 O3 Si2 -12.1(4) 7_755 .
O2 Na4 O3 Si2 168.3(3) . .
O5 Na4 O3 Si2 -142.8(3) 3_465 .
O3 Na4 O3 Si2 141.9(15) 4_645 .
Eu2 Na4 O3 Si2 -50.8(2) . .
Si1 Na4 O3 Si2 -177.7(5) . .
O6 Na4 O3 Na1 -8.09(16) 2_765 3_565
O6 Na4 O3 Na1 168.80(15) 3_465 3_565
O4 Na4 O3 Na1 -106.53(17) . 3_565
O1 Na4 O3 Na1 -106.8(2) 7_755 3_565
O2 Na4 O3 Na1 73.59(18) . 3_565
O5 Na4 O3 Na1 122.5(2) 3_465 3_565
O3 Na4 O3 Na1 47.2(16) 4_645 3_565
Eu2 Na4 O3 Na1 -145.55(11) . 3_565
Si2 Na4 O3 Na1 -94.7(3) . 3_565
Si1 Na4 O3 Na1 87.6(2) . 3_565
O6 Na4 O3 Na4 173.76(19) 2_765 4_655
O6 Na4 O3 Na4 -9.35(12) 3_465 4_655
O4 Na4 O3 Na4 75.31(15) . 4_655
O1 Na4 O3 Na4 75.0(2) 7_755 4_655
O2 Na4 O3 Na4 -104.6(2) . 4_655
O5 Na4 O3 Na4 -55.6(2) 3_465 4_655
O3 Na4 O3 Na4 -131.0(17) 4_645 4_655
Eu2 Na4 O3 Na4 36.30(10) . 4_655
Si2 Na4 O3 Na4 87.1(2) . 4_655
Si1 Na4 O3 Na4 -90.6(3) . 4_655
O6 Si2 O4 Eu1 5.3(5) . 3_565
O5 Si2 O4 Eu1 129.2(3) . 3_565
O3 Si2 O4 Eu1 -118.5(4) . 3_565
Na4 Si2 O4 Eu1 -101.6(4) . 3_565
Na1 Si2 O4 Eu1 -60.4(4) 3_565 3_565
Na4 Si2 O4 Eu1 65.6(4) 3_565 3_565
Na4 Si2 O4 Eu1 -176.1(4) 4_655 3_565
Eu3 Si2 O4 Eu1 109.6(4) . 3_565
Eu2 Si2 O4 Eu1 5.1(5) 3_565 3_565
O6 Si2 O4 Eu2 179.3(3) . .
O5 Si2 O4 Eu2 -56.8(4) . .
O3 Si2 O4 Eu2 55.5(4) . .
Na4 Si2 O4 Eu2 72.4(3) . .
Na1 Si2 O4 Eu2 113.6(3) 3_565 .
Na4 Si2 O4 Eu2 -120.4(3) 3_565 .
Na4 Si2 O4 Eu2 -2.1(3) 4_655 .
Eu3 Si2 O4 Eu2 -76.4(3) . .
Eu1 Si2 O4 Eu2 174.0(7) 3_565 .
Eu2 Si2 O4 Eu2 179.12(14) 3_565 .
O6 Si2 O4 Na4 107.0(3) . .
O5 Si2 O4 Na4 -129.15(15) . .
O3 Si2 O4 Na4 -16.8(3) . .
Na1 Si2 O4 Na4 41.21(18) 3_565 .
Na4 Si2 O4 Na4 167.23(10) 3_565 .
Na4 Si2 O4 Na4 -74.46(10) 4_655 .
Eu3 Si2 O4 Na4 -148.8(2) . .
Eu1 Si2 O4 Na4 101.6(4) 3_565 .
Eu2 Si2 O4 Na4 106.8(2) 3_565 .
O6 Si2 O4 Eu3 -104.3(3) . .
O5 Si2 O4 Eu3 19.6(2) . .
O3 Si2 O4 Eu3 131.9(2) . .
Na4 Si2 O4 Eu3 148.8(2) . .
Na1 Si2 O4 Eu3 -170.03(6) 3_565 .
Na4 Si2 O4 Eu3 -44.01(18) 3_565 .
Na4 Si2 O4 Eu3 74.29(12) 4_655 .
Eu1 Si2 O4 Eu3 -109.6(4) 3_565 .
Eu2 Si2 O4 Eu3 -104.5(2) 3_565 .
O6 Eu2 O4 Si2 151.5(5) 8_575 .
O6 Eu2 O4 Si2 -37.7(4) 3_465 .
O2 Eu2 O4 Si2 53.9(4) 7_765 .
O1 Eu2 O4 Si2 -137.8(4) 7_755 .
O4 Eu2 O4 Si2 144.2(3) 6 .
Na4 Eu2 O4 Si2 -179.0(3) 6 .
Na4 Eu2 O4 Si2 -79.4(3) . .
Eu3 Eu2 O4 Si2 85.4(3) . .
Na1 Eu2 O4 Si2 -0.7(5) . .
Na4 Eu2 O4 Si2 2.2(3) 4_655 .
Na4 Eu2 O4 Si2 98.5(4) 7_765 .
O6 Eu2 O4 Eu1 -32.7(6) 8_575 3_565
O6 Eu2 O4 Eu1 138.08(16) 3_465 3_565
O2 Eu2 O4 Eu1 -130.27(13) 7_765 3_565
O1 Eu2 O4 Eu1 38.02(12) 7_755 3_565
O4 Eu2 O4 Eu1 -39.97(17) 6 3_565
Na4 Eu2 O4 Eu1 -3.17(15) 6 3_565
Na4 Eu2 O4 Eu1 96.45(14) . 3_565
Eu3 Eu2 O4 Eu1 -98.82(13) . 3_565
Na1 Eu2 O4 Eu1 175.16(8) . 3_565
Na4 Eu2 O4 Eu1 178.01(15) 4_655 3_565
Na4 Eu2 O4 Eu1 -85.69(14) 7_765 3_565
O6 Eu2 O4 Na4 -129.1(6) 8_575 .
O6 Eu2 O4 Na4 41.62(15) 3_465 .
O2 Eu2 O4 Na4 133.27(11) 7_765 .
O1 Eu2 O4 Na4 -58.44(11) 7_755 .
O4 Eu2 O4 Na4 -136.42(8) 6 .
Na4 Eu2 O4 Na4 -99.62(12) 6 .
Eu3 Eu2 O4 Na4 164.73(13) . .
Na1 Eu2 O4 Na4 78.70(17) . .
Na4 Eu2 O4 Na4 81.55(7) 4_655 .
Na4 Eu2 O4 Na4 177.86(11) 7_765 .
O6 Eu2 O4 Eu3 66.1(6) 8_575 .
O6 Eu2 O4 Eu3 -123.10(14) 3_465 .
O2 Eu2 O4 Eu3 -31.46(10) 7_765 .
O1 Eu2 O4 Eu3 136.84(12) 7_755 .
O4 Eu2 O4 Eu3 58.85(11) 6 .
Na4 Eu2 O4 Eu3 95.65(9) 6 .
Na4 Eu2 O4 Eu3 -164.73(13) . .
Na1 Eu2 O4 Eu3 -86.02(15) . .
Na4 Eu2 O4 Eu3 -83.17(8) 4_655 .
Na4 Eu2 O4 Eu3 13.13(14) 7_765 .
O6 Na4 O4 Si2 -75.4(2) 2_765 .
O3 Na4 O4 Si2 12.1(2) . .
O6 Na4 O4 Si2 101.90(19) 3_465 .
O1 Na4 O4 Si2 -168.2(2) 7_755 .
O2 Na4 O4 Si2 12.2(3) . .
O5 Na4 O4 Si2 121.0(3) 3_465 .
O3 Na4 O4 Si2 -165.02(19) 4_645 .
Eu2 Na4 O4 Si2 138.1(2) . .
Si1 Na4 O4 Si2 19.02(18) . .
O6 Na4 O4 Eu1 61.37(19) 2_765 3_565
O3 Na4 O4 Eu1 148.8(2) . 3_565
O6 Na4 O4 Eu1 -121.33(16) 3_465 3_565
O1 Na4 O4 Eu1 -31.41(16) 7_755 3_565
O2 Na4 O4 Eu1 148.94(17) . 3_565
O5 Na4 O4 Eu1 -102.2(3) 3_465 3_565
O3 Na4 O4 Eu1 -28.3(2) 4_645 3_565
Eu2 Na4 O4 Eu1 -85.13(12) . 3_565
Si2 Na4 O4 Eu1 136.8(3) . 3_565
Si1 Na4 O4 Eu1 155.79(12) . 3_565
O6 Na4 O4 Eu2 146.51(17) 2_765 .
O3 Na4 O4 Eu2 -126.04(18) . .
O6 Na4 O4 Eu2 -36.20(12) 3_465 .
O1 Na4 O4 Eu2 53.72(14) 7_755 .
O2 Na4 O4 Eu2 -125.92(17) . .
O5 Na4 O4 Eu2 -17.1(3) 3_465 .
O3 Na4 O4 Eu2 56.88(19) 4_645 .
Si2 Na4 O4 Eu2 -138.1(2) . .
Si1 Na4 O4 Eu2 -119.07(9) . .
O6 Na4 O4 Eu3 174.2(3) 2_765 .
O3 Na4 O4 Eu3 -98.4(3) . .
O6 Na4 O4 Eu3 -8.5(3) 3_465 .
O1 Na4 O4 Eu3 81.4(3) 7_755 .
O2 Na4 O4 Eu3 -98.3(3) . .
O5 Na4 O4 Eu3 10.6(5) 3_465 .
O3 Na4 O4 Eu3 84.5(3) 4_645 .
Eu2 Na4 O4 Eu3 27.6(2) . .
Si2 Na4 O4 Eu3 -110.4(4) . .
Si1 Na4 O4 Eu3 -91.4(3) . .
O2 Eu3 O4 Si2 76.02(19) 3_565 .
O2 Eu3 O4 Si2 -103.98(19) 7_765 .
O4 Eu3 O4 Si2 166.66(12) 6 .
O4 Eu3 O4 Si2 -13.34(12) 2_775 .
O4 Eu3 O4 Si2 -113(93) 5_775 .
O5 Eu3 O4 Si2 166.66(12) 5_775 .
O5 Eu3 O4 Si2 -13.34(12) . .
Eu2 Eu3 O4 Si2 -137.0(2) . .
Eu2 Eu3 O4 Si2 43.0(2) 5_775 .
Si2 Eu3 O4 Si2 160.32(17) 6 .
Si2 Eu3 O4 Si2 -19.68(17) 2_775 .
O2 Eu3 O4 Eu1 -62.55(14) 3_565 3_565
O2 Eu3 O4 Eu1 117.45(14) 7_765 3_565
O4 Eu3 O4 Eu1 28.09(17) 6 3_565
O4 Eu3 O4 Eu1 -151.91(17) 2_775 3_565
O4 Eu3 O4 Eu1 109(100) 5_775 3_565
O5 Eu3 O4 Eu1 28.09(17) 5_775 3_565
O5 Eu3 O4 Eu1 -151.91(17) . 3_565
Eu2 Eu3 O4 Eu1 84.46(12) . 3_565
Eu2 Eu3 O4 Eu1 -95.54(12) 5_775 3_565
Si2 Eu3 O4 Eu1 21.74(13) 6 3_565
Si2 Eu3 O4 Eu1 -158.26(13) 2_775 3_565
O2 Eu3 O4 Eu2 -147.02(10) 3_565 .
O2 Eu3 O4 Eu2 32.98(10) 7_765 .
O4 Eu3 O4 Eu2 -56.37(12) 6 .
O4 Eu3 O4 Eu2 123.63(12) 2_775 .
O4 Eu3 O4 Eu2 24(72) 5_775 .
O5 Eu3 O4 Eu2 -56.37(12) 5_775 .
O5 Eu3 O4 Eu2 123.63(12) . .
Eu2 Eu3 O4 Eu2 180.0 5_775 .
Si2 Eu3 O4 Eu2 -62.72(8) 6 .
Si2 Eu3 O4 Eu2 117.28(8) 2_775 .
O2 Eu3 O4 Na4 -174.7(3) 3_565 .
O2 Eu3 O4 Na4 5.3(3) 7_765 .
O4 Eu3 O4 Na4 -84.1(3) 6 .
O4 Eu3 O4 Na4 95.9(3) 2_775 .
O4 Eu3 O4 Na4 -3(100) 5_775 .
O5 Eu3 O4 Na4 -84.1(3) 5_775 .
O5 Eu3 O4 Na4 95.9(3) . .
Eu2 Eu3 O4 Na4 -27.7(2) . .
Eu2 Eu3 O4 Na4 152.3(2) 5_775 .
Si2 Eu3 O4 Na4 -90.4(3) 6 .
Si2 Eu3 O4 Na4 89.6(3) 2_775 .
O6 Si2 O5 Si2 -71.5(2) . 2_775
O4 Si2 O5 Si2 160.73(18) . 2_775
O3 Si2 O5 Si2 48.8(2) . 2_775
Na4 Si2 O5 Si2 102.5(3) . 2_775
Na1 Si2 O5 Si2 -6.07(9) 3_565 2_775
Na4 Si2 O5 Si2 -91.8(2) 3_565 2_775
Na4 Si2 O5 Si2 91.7(2) 4_655 2_775
Eu3 Si2 O5 Si2 180.000(6) . 2_775
Eu1 Si2 O5 Si2 -175.89(6) 3_565 2_775
Eu2 Si2 O5 Si2 -50.61(5) 3_565 2_775
O6 Si2 O5 Eu3 108.5(2) . .
O4 Si2 O5 Eu3 -19.27(18) . .
O3 Si2 O5 Eu3 -131.2(2) . .
Na4 Si2 O5 Eu3 -77.5(3) . .
Na1 Si2 O5 Eu3 173.93(9) 3_565 .
Na4 Si2 O5 Eu3 88.22(19) 3_565 .
Na4 Si2 O5 Eu3 -88.3(2) 4_655 .
Eu1 Si2 O5 Eu3 4.11(6) 3_565 .
Eu2 Si2 O5 Eu3 129.39(5) 3_565 .
O6 Si2 O5 Na4 -163.2(2) . 4_655
O4 Si2 O5 Na4 69.0(3) . 4_655
O3 Si2 O5 Na4 -42.9(3) . 4_655
Na4 Si2 O5 Na4 10.8(5) . 4_655
Na1 Si2 O5 Na4 -97.76(18) 3_565 4_655
Na4 Si2 O5 Na4 176.5(4) 3_565 4_655
Eu3 Si2 O5 Na4 88.3(2) . 4_655
Eu1 Si2 O5 Na4 92.42(19) 3_565 4_655
Eu2 Si2 O5 Na4 -142.30(17) 3_565 4_655
O6 Si2 O5 Na4 20.2(4) . 3_565
O4 Si2 O5 Na4 -107.5(2) . 3_565
O3 Si2 O5 Na4 140.6(2) . 3_565
Na4 Si2 O5 Na4 -165.75(13) . 3_565
Na1 Si2 O5 Na4 85.7(2) 3_565 3_565
Na4 Si2 O5 Na4 -176.5(4) 4_655 3_565
Eu3 Si2 O5 Na4 -88.22(19) . 3_565
Eu1 Si2 O5 Na4 -84.1(2) 3_565 3_565
Eu2 Si2 O5 Na4 41.2(2) 3_565 3_565
O2 Eu3 O5 Si2 -78.03(15) 3_565 .
O2 Eu3 O5 Si2 101.97(15) 7_765 .
O4 Eu3 O5 Si2 13.13(12) 6 .
O4 Eu3 O5 Si2 -166.87(12) 2_775 .
O4 Eu3 O5 Si2 13.13(12) . .
O4 Eu3 O5 Si2 -166.87(12) 5_775 .
O5 Eu3 O5 Si2 87(100) 5_775 .
Eu2 Eu3 O5 Si2 53.04(5) . .
Eu2 Eu3 O5 Si2 -126.96(5) 5_775 .
Si2 Eu3 O5 Si2 0.000(2) 6 .
Si2 Eu3 O5 Si2 180.000(1) 2_775 .
O2 Eu3 O5 Si2 101.97(15) 3_565 2_775
O2 Eu3 O5 Si2 -78.03(15) 7_765 2_775
O4 Eu3 O5 Si2 -166.87(12) 6 2_775
O4 Eu3 O5 Si2 13.13(12) 2_775 2_775
O4 Eu3 O5 Si2 -166.87(12) . 2_775
O4 Eu3 O5 Si2 13.13(12) 5_775 2_775
O5 Eu3 O5 Si2 -93(100) 5_775 2_775
Eu2 Eu3 O5 Si2 -126.96(5) . 2_775
Eu2 Eu3 O5 Si2 53.04(5) 5_775 2_775
Si2 Eu3 O5 Si2 180.000(1) 6 2_775
O2 Eu3 O5 Na4 -168.47(15) 3_565 4_655
O2 Eu3 O5 Na4 11.53(15) 7_765 4_655
O4 Eu3 O5 Na4 -77.31(12) 6 4_655
O4 Eu3 O5 Na4 102.69(12) 2_775 4_655
O4 Eu3 O5 Na4 -77.31(12) . 4_655
O4 Eu3 O5 Na4 102.69(12) 5_775 4_655
O5 Eu3 O5 Na4 -4(100) 5_775 4_655
Eu2 Eu3 O5 Na4 -37.40(6) . 4_655
Eu2 Eu3 O5 Na4 142.60(6) 5_775 4_655
Si2 Eu3 O5 Na4 -90.44(7) 6 4_655
Si2 Eu3 O5 Na4 89.56(7) 2_775 4_655
O2 Eu3 O5 Na4 11.53(15) 3_565 3_565
O2 Eu3 O5 Na4 -168.47(15) 7_765 3_565
O4 Eu3 O5 Na4 102.69(12) 6 3_565
O4 Eu3 O5 Na4 -77.31(12) 2_775 3_565
O4 Eu3 O5 Na4 102.69(12) . 3_565
O4 Eu3 O5 Na4 -77.31(12) 5_775 3_565
O5 Eu3 O5 Na4 176(100) 5_775 3_565
Eu2 Eu3 O5 Na4 142.60(6) . 3_565
Eu2 Eu3 O5 Na4 -37.40(6) 5_775 3_565
Si2 Eu3 O5 Na4 89.56(7) 6 3_565
Si2 Eu3 O5 Na4 -90.44(7) 2_775 3_565
O4 Si2 O6 Na2 -179.7(4) . 3_565
O5 Si2 O6 Na2 59.4(6) . 3_565
O3 Si2 O6 Na2 -58.4(6) . 3_565
Na4 Si2 O6 Na2 -115.5(4) . 3_565
Na1 Si2 O6 Na2 -75.5(4) 3_565 3_565
Na4 Si2 O6 Na2 81.1(5) 3_565 3_565
Na4 Si2 O6 Na2 5.0(12) 4_655 3_565
Eu3 Si2 O6 Na2 119.6(4) . 3_565
Eu1 Si2 O6 Na2 -177.3(5) 3_565 3_565
Eu2 Si2 O6 Na2 0.000(1) 3_565 3_565
O4 Si2 O6 Eu2 -179.7(4) . 3_565
O5 Si2 O6 Eu2 59.4(6) . 3_565
O3 Si2 O6 Eu2 -58.4(6) . 3_565
Na4 Si2 O6 Eu2 -115.5(4) . 3_565
Na1 Si2 O6 Eu2 -75.5(4) 3_565 3_565
Na4 Si2 O6 Eu2 81.1(5) 3_565 3_565
Na4 Si2 O6 Eu2 5.0(12) 4_655 3_565
Eu3 Si2 O6 Eu2 119.6(4) . 3_565
Eu1 Si2 O6 Eu2 -177.3(5) 3_565 3_565
O4 Si2 O6 Na4 -7.8(5) . 2_765
O5 Si2 O6 Na4 -128.7(5) . 2_765
O3 Si2 O6 Na4 113.5(4) . 2_765
Na4 Si2 O6 Na4 56.4(4) . 2_765
Na1 Si2 O6 Na4 96.4(4) 3_565 2_765
Na4 Si2 O6 Na4 -107.1(4) 3_565 2_765
Na4 Si2 O6 Na4 176.9(4) 4_655 2_765
Eu3 Si2 O6 Na4 -68.5(4) . 2_765
Eu1 Si2 O6 Na4 -5.4(4) 3_565 2_765
Eu2 Si2 O6 Na4 171.9(8) 3_565 2_765
O4 Si2 O6 Na4 99.3(2) . 3_565
O5 Si2 O6 Na4 -21.7(4) . 3_565
O3 Si2 O6 Na4 -139.4(2) . 3_565
Na4 Si2 O6 Na4 163.46(8) . 3_565
Na1 Si2 O6 Na4 -156.6(2) 3_565 3_565
Na4 Si2 O6 Na4 -76.1(7) 4_655 3_565
Eu3 Si2 O6 Na4 38.5(2) . 3_565
Eu1 Si2 O6 Na4 101.62(13) 3_565 3_565
Eu2 Si2 O6 Na4 -81.1(5) 3_565 3_565
O4 Si2 O6 Na1 -104.2(2) . 3_565
O5 Si2 O6 Na1 134.9(3) . 3_565
O3 Si2 O6 Na1 17.1(2) . 3_565
Na4 Si2 O6 Na1 -39.99(19) . 3_565
Na4 Si2 O6 Na1 156.6(2) 3_565 3_565
Na4 Si2 O6 Na1 80.5(7) 4_655 3_565
Eu3 Si2 O6 Na1 -164.92(7) . 3_565
Eu1 Si2 O6 Na1 -101.83(10) 3_565 3_565
Eu2 Si2 O6 Na1 75.5(4) 3_565 3_565
